# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy1_a
_database_code_depnum_ccdc_archive 'CCDC 2168598'
loop_
_audit_author_name
_audit_author_address
'Dongdi Zhang'
;Henan University
China
;
_audit_update_record             
;
2022-04-25 deposited with the CCDC.	2022-05-24 downloaded from the CCDC.
;
_audit_creation_date             2021-07-30
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2016/6
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs Eu K O46 Se4 Ta6, 4(O)'
_chemical_formula_sum            'Cs Eu K O50 Se4 Ta6'
_chemical_formula_weight         2525.51
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.3382(7)
_cell_length_b                   27.3560(15)
_cell_length_c                   14.0173(8)
_cell_angle_alpha                90
_cell_angle_beta                 113.7870(10)
_cell_angle_gamma                90
_cell_volume                     4329.3(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    3879
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.62
_cell_measurement_theta_min      2.34
_shelx_estimated_absorpt_T_max   0.207
_shelx_estimated_absorpt_T_min   0.157
_exptl_absorpt_coefficient_mu    20.945
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4393
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1183 before and 0.0526 after correction.
The Ratio of minimum to maximum transmission is 0.5891.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.875
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4444
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.11
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0529
_diffrn_reflns_av_unetI/netI     0.0610
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22421
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.754
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6011
_reflns_number_total             7699
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         2.425
_refine_diff_density_min         -4.258
_refine_diff_density_rms         0.347
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7699
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0606
_refine_ls_R_factor_gt           0.0421
_refine_ls_restrained_S_all      1.023
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0349P)²+97.8519P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0920
_refine_ls_wR_factor_ref         0.1007
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     iterative
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28609(5) 0.54915(2) 0.55607(4) 0.01213(14) Uani 1 1 d . . . . .
Ta2 Ta 0.43731(5) 0.65820(2) 0.47083(4) 0.01202(14) Uani 1 1 d . . . . .
Ta3 Ta 0.17314(5) 0.60808(2) 0.32947(4) 0.01261(14) Uani 1 1 d . . . . .
Ta4 Ta 0.13772(5) 0.64086(2) 0.66540(4) 0.01231(14) Uani 1 1 d . . . . .
Ta5 Ta 0.28318(5) 0.75184(2) 0.57610(4) 0.01303(14) Uani 1 1 d . . . . .
Ta6 Ta 0.03335(5) 0.70153(2) 0.43995(4) 0.01523(15) Uani 1 1 d . . . . .
Eu1 Eu 0.68504(7) 0.64926(3) 0.98655(6) 0.01793(18) Uani 1 1 d . . . . .
Se1 Se 0.41791(13) 0.53782(5) 0.38211(11) 0.0166(3) Uani 1 1 d . . . . .
Se2 Se 0.05142(13) 0.76030(5) 0.66103(11) 0.0171(3) Uani 1 1 d . . . . .
Se3 Se 0.37646(13) 0.71163(5) 0.82816(11) 0.0152(3) Uani 1 1 d . . . . .
Se4 Se 0.49174(14) 0.62401(6) 0.71343(12) 0.0210(3) Uani 1 1 d . . . . .
Cs1 Cs -0.18129(13) 0.66447(6) 0.71926(13) 0.0625(4) Uani 1 1 d . . . . .
K1 K 0.2243(4) 0.57346(17) 0.0691(4) 0.0527(13) Uani 1 1 d . . . . .
O2 O 0.6185(9) 0.6138(4) 0.8152(8) 0.025(3) Uiso 1 1 d . . . . .
O3 O 0.3880(12) 0.8012(5) 0.5518(10) 0.046(3) Uiso 1 1 d . . . . .
O4 O -0.1356(10) 0.6940(4) 0.3456(8) 0.029(3) Uiso 1 1 d . . . . .
O5 O 0.5058(9) 0.6877(4) 0.8970(8) 0.023(2) Uiso 1 1 d . . . . .
O6 O 0.5025(9) 0.6929(4) 0.3829(8) 0.023(2) Uiso 1 1 d . . . . .
O7 O 0.5940(9) 0.6855(4) 0.4901(8) 0.024(2) Uiso 1 1 d . . . . .
O8 O -0.0788(10) 0.7371(4) 0.3173(8) 0.025(3) Uiso 1 1 d . . . . .
O9 O 0.0962(9) 0.6194(4) 0.1773(8) 0.025(3) Uiso 1 1 d . . . . .
O10 O 0.5434(9) 0.6379(4) 0.6205(8) 0.021(2) Uiso 1 1 d . . . . .
O11 O 0.1256(9) 0.6051(4) 0.7846(8) 0.025(2) Uiso 1 1 d . . . . .
O12 O 0.3181(12) 0.8215(5) 0.6032(10) 0.044(3) Uiso 1 1 d . . . . .
O13 O 0.0341(10) 0.5805(4) 0.2130(8) 0.025(3) Uiso 1 1 d . . . . .
O14 O 0.0718(9) 0.7030(4) 0.7110(8) 0.020(2) Uiso 1 1 d . . . . .
O15 O 0.0170(9) 0.6001(4) 0.6866(8) 0.022(2) Uiso 1 1 d . . . . .
O16 O 0.2964(9) 0.6592(4) 0.7835(8) 0.022(2) Uiso 1 1 d . . . . .
O17 O 0.2009(9) 0.4871(4) 0.5509(8) 0.023(2) Uiso 1 1 d . . . . .
O18 O 0.4002(8) 0.7280(3) 0.7193(7) 0.015(2) Uiso 1 1 d . . . . .
O19 O 0.3174(9) 0.4898(4) 0.6447(8) 0.023(2) Uiso 1 1 d . . . . .
O20 O 0.0868(9) 0.6574(3) 0.3638(7) 0.017(2) Uiso 1 1 d . . . . .
O21 O 0.2827(9) 0.5581(4) 0.2968(8) 0.019(2) Uiso 1 1 d . . . . .
O22 O -0.0253(9) 0.7486(4) 0.5325(8) 0.022(2) Uiso 1 1 d . . . . .
O23 O 0.2095(8) 0.5876(3) 0.6228(7) 0.014(2) Uiso 1 1 d . . . . .
O24 O 0.1879(9) 0.7762(4) 0.6673(8) 0.021(2) Uiso 1 1 d . . . . .
O25 O 0.4486(9) 0.5655(4) 0.6755(7) 0.018(2) Uiso 1 1 d . . . . .
O26 O 0.3838(9) 0.5179(3) 0.4823(7) 0.017(2) Uiso 1 1 d . . . . .
O27 O 0.3731(9) 0.7091(4) 0.5175(8) 0.020(2) Uiso 1 1 d . . . . .
O28 O 0.4928(9) 0.5906(3) 0.4274(7) 0.016(2) Uiso 1 1 d . . . . .
O29 O 0.1443(9) 0.7560(4) 0.4481(8) 0.020(2) Uiso 1 1 d . . . . .
O30 O -0.0056(9) 0.6456(4) 0.5210(8) 0.019(2) Uiso 1 1 d . . . . .
O31 O 0.1408(9) 0.5547(3) 0.4152(7) 0.017(2) Uiso 1 1 d . . . . .
O32 O 0.1815(9) 0.6897(3) 0.5767(7) 0.017(2) Uiso 1 1 d . . . . .
O33 O 0.2935(9) 0.6587(3) 0.3254(7) 0.018(2) Uiso 1 1 d . . . . .
O34 O 0.3098(8) 0.6092(3) 0.4786(7) 0.012(2) Uiso 1 1 d . . . . .
O35 O 0.5628(11) 0.6364(4) 1.0852(9) 0.034(3) Uiso 1 1 d . . . . .
O36 O 0.6989(11) 0.7276(4) 1.0830(9) 0.036(3) Uiso 1 1 d . . . . .
O37 O 0.8322(11) 0.6390(5) 1.1634(9) 0.040(3) Uiso 1 1 d . . . . .
O1 O 0.7613(11) 0.7117(4) 0.9096(9) 0.038(3) Uiso 1 1 d . . . . .
O38 O -0.0427(11) 0.4989(5) 0.3472(10) 0.042(3) Uiso 1 1 d . . . . .
O39 O 0.6267(12) 0.7682(5) 0.7521(10) 0.049(4) Uiso 1 1 d . . . . .
O40 O -0.2153(14) 0.6129(6) 0.4977(12) 0.067(4) Uiso 1 1 d . . . . .
O41 O 0.0514(14) 0.6462(6) 0.9265(12) 0.063(4) Uiso 1 1 d . . . . .
O42 O 0.8653(13) 0.6153(5) 0.9766(11) 0.052(4) Uiso 1 1 d . . . . .
O43 O 0.6777(12) 0.5631(5) 1.0089(10) 0.049(4) Uiso 1 1 d . . . . .
O44 O 0.5812(13) 0.4981(5) 0.8444(11) 0.060(4) Uiso 1 1 d . . . . .
O45 O 0.3620(14) 0.5813(6) -0.0573(12) 0.069(5) Uiso 1 1 d . . . . .
O46 O 0.0920(15) 0.5147(6) -0.1063(13) 0.072(5) Uiso 1 1 d . . . . .
O47 O 0.3543(15) 0.4937(6) 0.8519(13) 0.078(5) Uiso 1 1 d . . . . .
O48 O 0.6004(19) 0.6133(7) 1.2805(16) 0.102(7) Uiso 1 1 d . . . . .
O49 O 0.276(3) 0.4406(11) 0.332(2) 0.160(10) Uiso 1 1 d . . . . .
O50 O 0.142(2) 0.4695(9) 0.1323(19) 0.131(8) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3255(8) . ?
Ta1 O17 1.982(10) . ?
Ta1 O19 1.985(10) . ?
Ta1 O23 1.894(9) . ?
Ta1 O25 2.077(10) . ?
Ta1 O26 2.064(10) . ?
Ta1 O31 2.069(10) . ?
Ta1 O34 2.053(9) . ?
Ta2 Ta3 3.3496(8) . ?
Ta2 O6 1.966(10) . ?
Ta2 O7 1.987(11) . ?
Ta2 O10 2.051(10) . ?
Ta2 O27 1.848(10) . ?
Ta2 O28 2.144(9) . ?
Ta2 O33 2.095(10) . ?
Ta2 O34 2.104(9) . ?
Ta3 K1 4.059(5) . ?
Ta3 O9 1.978(10) . ?
Ta3 O13 1.979(11) . ?
Ta3 O20 1.897(10) . ?
Ta3 O21 2.099(10) . ?
Ta3 O31 2.030(10) . ?
Ta3 O33 2.048(10) . ?
Ta3 O34 2.091(9) . ?
Ta4 Ta6 3.3342(8) . ?
Ta4 Cs1 4.3449(16) . ?
Ta4 O11 1.993(10) . ?
Ta4 O14 2.093(10) . ?
Ta4 O15 1.977(10) . ?
Ta4 O16 2.052(10) . ?
Ta4 O23 1.921(9) . ?
Ta4 O30 2.086(10) . ?
Ta4 O32 2.042(10) . ?
Ta5 Ta6 3.2081(9) . ?
Ta5 O3 1.992(13) . ?
Ta5 O12 1.958(13) . ?
Ta5 O18 2.049(9) . ?
Ta5 O24 2.162(10) . ?
Ta5 O27 2.001(10) . ?
Ta5 O29 1.920(10) . ?
Ta5 O32 2.114(10) . ?
Ta6 O4 1.978(11) . ?
Ta6 O8 1.975(11) . ?
Ta6 O20 1.898(10) . ?
Ta6 O22 2.149(10) . ?
Ta6 O29 1.995(10) . ?
Ta6 O30 2.076(10) . ?
Ta6 O32 2.072(10) . ?
Eu1 Se4 3.6683(17) . ?
Eu1 Cs1 4.6813(18) 1_655 ?
Eu1 O2 2.407(10) . ?
Eu1 O5 2.309(11) . ?
Eu1 O35 2.448(12) . ?
Eu1 O36 2.503(12) . ?
Eu1 O37 2.427(12) . ?
Eu1 O1 2.404(12) . ?
Eu1 O42 2.466(14) . ?
Eu1 O43 2.385(14) . ?
Se1 O21 1.706(10) . ?
Se1 O26 1.710(10) . ?
Se1 O28 1.693(10) . ?
Se2 Cs1 4.204(2) . ?
Se2 O14 1.693(10) . ?
Se2 O22 1.694(10) . ?
Se2 O24 1.707(10) . ?
Se3 O5 1.632(11) . ?
Se3 O16 1.711(10) . ?
Se3 O18 1.726(9) . ?
Se4 Cs1 4.152(2) 1_655 ?
Se4 O2 1.661(11) . ?
Se4 O10 1.708(10) . ?
Se4 O25 1.703(10) . ?
Cs1 O2 3.537(11) 1_455 ?
Cs1 O7 3.340(11) 1_455 ?
Cs1 O8 3.055(11) 4_576 ?
Cs1 O10 3.192(10) 1_455 ?
Cs1 O14 3.341(10) . ?
Cs1 O15 3.194(10) . ?
Cs1 O36 3.503(12) 4_475 ?
Cs1 O1 3.289(12) 1_455 ?
Cs1 O40 3.280(16) . ?
Cs1 O41 3.194(16) . ?
Cs1 O42 3.671(14) 1_455 ?
Cs1 O49 3.08(3) 3_566 ?
K1 O9 2.884(11) . ?
K1 O12 3.061(14) 4_575 ?
K1 O21 3.004(11) . ?
K1 O41 3.011(16) 1_554 ?
K1 O44 2.952(16) 3_666 ?
K1 O45 2.915(17) . ?
K1 O46 2.839(17) . ?
K1 O50 3.26(2) . ?
O3 O12 1.440(17) . ?
O4 O8 1.504(15) . ?
O6 O7 1.485(14) . ?
O9 O13 1.511(14) . ?
O11 O15 1.489(14) . ?
O17 O19 1.509(14) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O17 Ta1 Ta3 111.6(3) . . ?
O17 Ta1 O19 44.7(4) . . ?
O17 Ta1 O25 122.6(4) . . ?
O17 Ta1 O26 92.0(4) . . ?
O17 Ta1 O31 77.6(4) . . ?
O17 Ta1 O34 148.4(4) . . ?
O19 Ta1 Ta3 153.5(3) . . ?
O19 Ta1 O25 77.9(4) . . ?
O19 Ta1 O26 88.2(4) . . ?
O19 Ta1 O31 122.2(4) . . ?
O19 Ta1 O34 162.1(4) . . ?
O23 Ta1 Ta3 95.9(3) . . ?
O23 Ta1 O17 97.5(4) . . ?
O23 Ta1 O19 98.9(4) . . ?
O23 Ta1 O25 89.7(4) . . ?
O23 Ta1 O26 170.5(4) . . ?
O23 Ta1 O31 91.0(4) . . ?
O23 Ta1 O34 91.3(4) . . ?
O25 Ta1 Ta3 124.2(3) . . ?
O26 Ta1 Ta3 80.0(3) . . ?
O26 Ta1 O25 85.6(4) . . ?
O26 Ta1 O31 90.5(4) . . ?
O31 Ta1 Ta3 35.4(3) . . ?
O31 Ta1 O25 159.5(4) . . ?
O34 Ta1 Ta3 37.0(3) . . ?
O34 Ta1 O25 87.5(4) . . ?
O34 Ta1 O26 80.2(4) . . ?
O34 Ta1 O31 71.9(4) . . ?
O6 Ta2 Ta3 111.9(3) . . ?
O6 Ta2 O7 44.1(4) . . ?
O6 Ta2 O10 121.2(4) . . ?
O6 Ta2 O28 88.8(4) . . ?
O6 Ta2 O33 77.7(4) . . ?
O6 Ta2 O34 147.5(4) . . ?
O7 Ta2 Ta3 153.6(3) . . ?
O7 Ta2 O10 77.2(4) . . ?
O7 Ta2 O28 87.6(4) . . ?
O7 Ta2 O33 121.7(4) . . ?
O7 Ta2 O34 160.0(4) . . ?
O10 Ta2 Ta3 124.2(3) . . ?
O10 Ta2 O28 85.0(4) . . ?
O10 Ta2 O33 159.7(4) . . ?
O10 Ta2 O34 87.5(4) . . ?
O27 Ta2 Ta3 93.7(3) . . ?
O27 Ta2 O6 101.6(4) . . ?
O27 Ta2 O7 101.6(4) . . ?
O27 Ta2 O10 91.7(4) . . ?
O27 Ta2 O28 169.3(4) . . ?
O27 Ta2 O33 91.4(4) . . ?
O27 Ta2 O34 91.5(4) . . ?
O28 Ta2 Ta3 79.9(3) . . ?
O33 Ta2 Ta3 35.6(3) . . ?
O33 Ta2 O28 88.3(4) . . ?
O33 Ta2 O34 72.4(4) . . ?
O34 Ta2 Ta3 36.9(2) . . ?
O34 Ta2 O28 78.2(4) . . ?
Ta1 Ta3 Ta2 72.571(18) . . ?
Ta1 Ta3 K1 126.04(6) . . ?
Ta2 Ta3 K1 99.22(8) . . ?
O9 Ta3 Ta1 160.0(3) . . ?
O9 Ta3 Ta2 120.2(3) . . ?
O9 Ta3 K1 41.3(3) . . ?
O9 Ta3 O13 44.9(4) . . ?
O9 Ta3 O21 86.5(4) . . ?
O9 Ta3 O31 128.9(4) . . ?
O9 Ta3 O33 84.4(4) . . ?
O9 Ta3 O34 156.7(4) . . ?
O13 Ta3 Ta1 119.5(3) . . ?
O13 Ta3 Ta2 163.1(3) . . ?
O13 Ta3 K1 64.3(3) . . ?
O13 Ta3 O21 89.6(4) . . ?
O13 Ta3 O31 84.4(4) . . ?
O13 Ta3 O33 129.2(4) . . ?
O13 Ta3 O34 155.7(4) . . ?
O20 Ta3 Ta1 99.5(3) . . ?
O20 Ta3 Ta2 94.0(3) . . ?
O20 Ta3 K1 134.5(3) . . ?
O20 Ta3 O9 95.0(4) . . ?
O20 Ta3 O13 95.3(4) . . ?
O20 Ta3 O21 174.4(4) . . ?
O20 Ta3 O31 95.6(4) . . ?
O20 Ta3 O33 90.8(4) . . ?
O20 Ta3 O34 92.6(4) . . ?
O21 Ta3 Ta1 80.5(3) . . ?
O21 Ta3 Ta2 80.6(3) . . ?
O21 Ta3 K1 45.9(3) . . ?
O31 Ta3 Ta1 36.2(3) . . ?
O31 Ta3 Ta2 108.7(3) . . ?
O31 Ta3 K1 120.2(3) . . ?
O31 Ta3 O21 87.7(4) . . ?
O31 Ta3 O33 145.1(4) . . ?
O31 Ta3 O34 71.9(4) . . ?
O33 Ta3 Ta1 109.0(3) . . ?
O33 Ta3 Ta2 36.5(3) . . ?
O33 Ta3 K1 75.8(3) . . ?
O33 Ta3 O21 84.0(4) . . ?
O33 Ta3 O34 73.6(4) . . ?
O34 Ta3 Ta1 36.2(2) . . ?
O34 Ta3 Ta2 37.1(2) . . ?
O34 Ta3 K1 123.2(3) . . ?
O34 Ta3 O21 84.1(4) . . ?
Ta6 Ta4 Cs1 93.44(3) . . ?
O11 Ta4 Ta6 155.2(3) . . ?
O11 Ta4 Cs1 63.1(3) . . ?
O11 Ta4 O14 88.5(4) . . ?
O11 Ta4 O16 79.3(4) . . ?
O11 Ta4 O30 121.5(4) . . ?
O11 Ta4 O32 163.7(4) . . ?
O14 Ta4 Ta6 80.6(3) . . ?
O14 Ta4 Cs1 48.3(3) . . ?
O15 Ta4 Ta6 113.4(3) . . ?
O15 Ta4 Cs1 42.9(3) . . ?
O15 Ta4 O11 44.1(4) . . ?
O15 Ta4 O14 90.2(4) . . ?
O15 Ta4 O16 123.2(4) . . ?
O15 Ta4 O30 77.6(4) . . ?
O15 Ta4 O32 149.5(4) . . ?
O16 Ta4 Ta6 121.4(3) . . ?
O16 Ta4 Cs1 117.4(3) . . ?
O16 Ta4 O14 85.2(4) . . ?
O16 Ta4 O30 158.0(4) . . ?
O23 Ta4 Ta6 97.7(3) . . ?
O23 Ta4 Cs1 136.9(3) . . ?
O23 Ta4 O11 95.0(4) . . ?
O23 Ta4 O14 174.8(4) . . ?
O23 Ta4 O15 95.1(4) . . ?
O23 Ta4 O16 91.5(4) . . ?
O23 Ta4 O30 93.6(4) . . ?
O23 Ta4 O32 92.2(4) . . ?
O30 Ta4 Ta6 36.7(3) . . ?
O30 Ta4 Cs1 71.7(3) . . ?
O30 Ta4 O14 87.9(4) . . ?
O32 Ta4 Ta6 36.2(3) . . ?
O32 Ta4 Cs1 119.3(3) . . ?
O32 Ta4 O14 83.4(4) . . ?
O32 Ta4 O16 86.0(4) . . ?
O32 Ta4 O30 72.4(4) . . ?
O3 Ta5 Ta6 136.3(4) . . ?
O3 Ta5 O18 97.7(5) . . ?
O3 Ta5 O24 115.9(5) . . ?
O3 Ta5 O27 79.6(5) . . ?
O3 Ta5 O32 166.6(5) . . ?
O12 Ta5 Ta6 128.1(4) . . ?
O12 Ta5 O3 42.7(5) . . ?
O12 Ta5 O18 96.1(5) . . ?
O12 Ta5 O24 73.4(5) . . ?
O12 Ta5 O27 122.2(5) . . ?
O12 Ta5 O32 150.0(5) . . ?
O18 Ta5 Ta6 125.1(3) . . ?
O18 Ta5 O24 81.7(4) . . ?
O18 Ta5 O32 85.7(4) . . ?
O24 Ta5 Ta6 82.1(3) . . ?
O27 Ta5 Ta6 93.7(3) . . ?
O27 Ta5 O18 85.9(4) . . ?
O27 Ta5 O24 161.2(4) . . ?
O27 Ta5 O32 87.7(4) . . ?
O29 Ta5 Ta6 35.8(3) . . ?
O29 Ta5 O3 101.3(5) . . ?
O29 Ta5 O12 99.6(5) . . ?
O29 Ta5 O18 160.8(4) . . ?
O29 Ta5 O24 92.4(4) . . ?
O29 Ta5 O27 94.9(4) . . ?
O29 Ta5 O32 75.2(4) . . ?
O32 Ta5 Ta6 39.5(3) . . ?
O32 Ta5 O24 77.3(4) . . ?
Ta5 Ta6 Ta4 74.847(19) . . ?
O4 Ta6 Ta4 118.8(3) . . ?
O4 Ta6 Ta5 160.5(3) . . ?
O4 Ta6 O22 86.8(4) . . ?
O4 Ta6 O29 129.0(4) . . ?
O4 Ta6 O30 82.8(4) . . ?
O4 Ta6 O32 154.3(4) . . ?
O8 Ta6 Ta4 159.7(3) . . ?
O8 Ta6 Ta5 118.3(3) . . ?
O8 Ta6 O4 44.7(4) . . ?
O8 Ta6 O22 86.6(4) . . ?
O8 Ta6 O29 84.6(4) . . ?
O8 Ta6 O30 127.2(4) . . ?
O8 Ta6 O32 158.3(4) . . ?
O20 Ta6 Ta4 97.3(3) . . ?
O20 Ta6 Ta5 98.0(3) . . ?
O20 Ta6 O4 94.0(4) . . ?
O20 Ta6 O8 96.0(4) . . ?
O20 Ta6 O22 177.0(4) . . ?
O20 Ta6 O29 96.9(4) . . ?
O20 Ta6 O30 92.8(4) . . ?
O20 Ta6 O32 92.5(4) . . ?
O22 Ta6 Ta4 79.7(3) . . ?
O22 Ta6 Ta5 82.0(3) . . ?
O29 Ta6 Ta4 108.9(3) . . ?
O29 Ta6 Ta5 34.2(3) . . ?
O29 Ta6 O22 84.8(4) . . ?
O29 Ta6 O30 145.5(4) . . ?
O29 Ta6 O32 74.6(4) . . ?
O30 Ta6 Ta4 36.9(3) . . ?
O30 Ta6 Ta5 111.7(3) . . ?
O30 Ta6 O22 84.4(4) . . ?
O32 Ta6 Ta4 35.6(3) . . ?
O32 Ta6 Ta5 40.4(3) . . ?
O32 Ta6 O22 85.5(4) . . ?
O32 Ta6 O30 72.0(4) . . ?
Se4 Eu1 Cs1 58.14(3) . 1_655 ?
O2 Eu1 Se4 21.0(3) . . ?
O2 Eu1 Cs1 47.6(3) . 1_655 ?
O2 Eu1 O35 117.8(4) . . ?
O2 Eu1 O36 143.7(4) . . ?
O2 Eu1 O37 141.8(4) . . ?
O2 Eu1 O42 75.2(4) . . ?
O5 Eu1 Se4 56.1(3) . . ?
O5 Eu1 Cs1 95.4(3) . 1_655 ?
O5 Eu1 O2 77.0(4) . . ?
O5 Eu1 O35 72.5(4) . . ?
O5 Eu1 O36 75.2(4) . . ?
O5 Eu1 O37 140.0(4) . . ?
O5 Eu1 O1 84.0(4) . . ?
O5 Eu1 O42 146.0(4) . . ?
O5 Eu1 O43 116.3(4) . . ?
O35 Eu1 Se4 105.9(3) . . ?
O35 Eu1 Cs1 164.0(3) . 1_655 ?
O35 Eu1 O36 75.0(4) . . ?
O35 Eu1 O42 138.9(4) . . ?
O36 Eu1 Se4 126.8(3) . . ?
O36 Eu1 Cs1 112.8(3) . 1_655 ?
O37 Eu1 Se4 161.4(3) . . ?
O37 Eu1 Cs1 117.9(3) . 1_655 ?
O37 Eu1 O35 77.5(4) . . ?
O37 Eu1 O36 71.8(4) . . ?
O37 Eu1 O42 72.2(4) . . ?
O1 Eu1 Se4 82.7(3) . . ?
O1 Eu1 Cs1 41.4(3) . 1_655 ?
O1 Eu1 O2 82.9(4) . . ?
O1 Eu1 O35 142.8(4) . . ?
O1 Eu1 O36 71.4(4) . . ?
O1 Eu1 O37 105.9(4) . . ?
O1 Eu1 O42 73.5(4) . . ?
O42 Eu1 Se4 95.3(3) . . ?
O42 Eu1 Cs1 51.0(3) . 1_655 ?
O42 Eu1 O36 119.1(4) . . ?
O43 Eu1 Se4 84.7(3) . . ?
O43 Eu1 Cs1 103.7(3) . 1_655 ?
O43 Eu1 O2 73.6(4) . . ?
O43 Eu1 O35 73.7(4) . . ?
O43 Eu1 O36 140.7(4) . . ?
O43 Eu1 O37 78.7(4) . . ?
O43 Eu1 O1 143.4(4) . . ?
O43 Eu1 O42 73.6(5) . . ?
O21 Se1 O26 100.6(5) . . ?
O28 Se1 O21 102.5(5) . . ?
O28 Se1 O26 104.0(5) . . ?
O14 Se2 Cs1 48.8(4) . . ?
O14 Se2 O22 101.0(5) . . ?
O14 Se2 O24 103.7(5) . . ?
O22 Se2 Cs1 87.5(4) . . ?
O22 Se2 O24 102.7(5) . . ?
O24 Se2 Cs1 152.4(3) . . ?
O5 Se3 O16 99.4(5) . . ?
O5 Se3 O18 98.8(5) . . ?
O16 Se3 O18 100.0(5) . . ?
Eu1 Se4 Cs1 73.24(4) . 1_655 ?
O2 Se4 Eu1 31.2(4) . . ?
O2 Se4 Cs1 57.1(4) . 1_655 ?
O2 Se4 O10 100.4(5) . . ?
O2 Se4 O25 100.3(5) . . ?
O10 Se4 Eu1 117.9(3) . . ?
O10 Se4 Cs1 45.3(3) . 1_655 ?
O25 Se4 Eu1 119.5(3) . . ?
O25 Se4 Cs1 115.8(3) . 1_655 ?
O25 Se4 O10 97.9(5) . . ?
O2 Cs1 O42 48.7(3) 1_455 1_455 ?
O7 Cs1 O2 89.8(3) 1_455 1_455 ?
O7 Cs1 O14 109.7(3) 1_455 . ?
O7 Cs1 O36 47.7(3) 1_455 4_475 ?
O7 Cs1 O42 138.5(3) 1_455 1_455 ?
O8 Cs1 O2 113.6(3) 4_576 1_455 ?
O8 Cs1 O7 108.3(3) 4_576 1_455 ?
O8 Cs1 O10 124.8(3) 4_576 1_455 ?
O8 Cs1 O14 61.0(3) 4_576 . ?
O8 Cs1 O15 110.4(3) 4_576 . ?
O8 Cs1 O36 60.7(3) 4_576 4_475 ?
O8 Cs1 O1 58.3(3) 4_576 1_455 ?
O8 Cs1 O40 132.6(3) 4_576 . ?
O8 Cs1 O41 70.8(3) 4_576 . ?
O8 Cs1 O42 90.5(3) 4_576 1_455 ?
O8 Cs1 O49 167.9(6) 4_576 3_566 ?
O10 Cs1 O2 44.9(2) 1_455 1_455 ?
O10 Cs1 O7 45.3(3) 1_455 1_455 ?
O10 Cs1 O14 154.5(3) 1_455 . ?
O10 Cs1 O15 123.7(3) 1_455 . ?
O10 Cs1 O36 79.3(3) 1_455 4_475 ?
O10 Cs1 O1 84.3(3) 1_455 1_455 ?
O10 Cs1 O40 77.5(3) 1_455 . ?
O10 Cs1 O41 140.1(3) 1_455 . ?
O10 Cs1 O42 93.5(3) 1_455 1_455 ?
O14 Cs1 O2 160.5(2) . 1_455 ?
O14 Cs1 O36 84.8(3) . 4_475 ?
O14 Cs1 O42 111.8(3) . 1_455 ?
O15 Cs1 O2 122.1(3) . 1_455 ?
O15 Cs1 O7 110.1(3) . 1_455 ?
O15 Cs1 O14 52.3(3) . . ?
O15 Cs1 O36 124.4(3) . 4_475 ?
O15 Cs1 O1 139.6(3) . 1_455 ?
O15 Cs1 O40 55.9(3) . . ?
O15 Cs1 O41 65.4(3) . . ?
O15 Cs1 O42 96.5(3) . 1_455 ?
O36 Cs1 O2 109.4(3) 4_475 1_455 ?
O36 Cs1 O42 135.1(3) 4_475 1_455 ?
O1 Cs1 O2 55.5(3) 1_455 1_455 ?
O1 Cs1 O7 110.2(3) 1_455 1_455 ?
O1 Cs1 O14 114.5(3) 1_455 . ?
O1 Cs1 O36 86.0(3) 1_455 4_475 ?
O1 Cs1 O42 49.2(3) 1_455 1_455 ?
O40 Cs1 O2 110.4(3) . 1_455 ?
O40 Cs1 O7 54.8(3) . 1_455 ?
O40 Cs1 O14 82.4(3) . . ?
O40 Cs1 O36 89.0(3) . 4_475 ?
O40 Cs1 O1 161.8(4) . 1_455 ?
O40 Cs1 O42 133.0(3) . 1_455 ?
O41 Cs1 O2 95.9(3) . 1_455 ?
O41 Cs1 O7 174.1(3) . 1_455 ?
O41 Cs1 O14 64.6(3) . . ?
O41 Cs1 O36 130.9(3) . 4_475 ?
O41 Cs1 O1 74.5(4) . 1_455 ?
O41 Cs1 O40 121.2(4) . . ?
O41 Cs1 O42 47.3(4) . 1_455 ?
O49 Cs1 O2 57.7(6) 3_566 1_455 ?
O49 Cs1 O7 81.1(6) 3_566 1_455 ?
O49 Cs1 O10 56.5(6) 3_566 1_455 ?
O49 Cs1 O14 124.0(6) 3_566 . ?
O49 Cs1 O15 72.1(6) 3_566 . ?
O49 Cs1 O36 128.5(6) 3_566 4_475 ?
O49 Cs1 O1 111.7(6) 3_566 1_455 ?
O49 Cs1 O40 59.0(6) 3_566 . ?
O49 Cs1 O41 100.6(6) 3_566 . ?
O49 Cs1 O42 77.4(6) 3_566 1_455 ?
O9 K1 Ta3 26.9(2) . . ?
O9 K1 O12 76.2(3) . 4_575 ?
O9 K1 O21 56.6(3) . . ?
O9 K1 O41 70.7(4) . 1_554 ?
O9 K1 O44 126.9(4) . 3_666 ?
O9 K1 O45 149.9(4) . . ?
O9 K1 O50 86.6(5) . . ?
O12 K1 Ta3 80.0(3) 4_575 . ?
O12 K1 O50 156.3(5) 4_575 . ?
O21 K1 Ta3 30.1(2) . . ?
O21 K1 O12 93.0(3) . 4_575 ?
O21 K1 O41 126.8(4) . 1_554 ?
O21 K1 O50 63.7(5) . . ?
O41 K1 Ta3 96.7(3) 1_554 . ?
O41 K1 O12 66.8(4) 1_554 4_575 ?
O41 K1 O50 122.8(6) 1_554 . ?
O44 K1 Ta3 100.5(3) 3_666 . ?
O44 K1 O12 111.4(4) 3_666 4_575 ?
O44 K1 O21 70.4(4) 3_666 . ?
O44 K1 O41 162.1(5) 3_666 1_554 ?
O44 K1 O50 66.5(5) 3_666 . ?
O45 K1 Ta3 150.4(4) . . ?
O45 K1 O12 75.5(4) . 4_575 ?
O45 K1 O21 135.0(4) . . ?
O45 K1 O41 88.7(5) . 1_554 ?
O45 K1 O44 73.9(4) . 3_666 ?
O45 K1 O50 123.5(6) . . ?
O46 K1 Ta3 131.9(4) . . ?
O46 K1 O9 117.2(4) . . ?
O46 K1 O12 135.7(4) . 4_575 ?
O46 K1 O21 130.5(4) . . ?
O46 K1 O41 78.0(5) . 1_554 ?
O46 K1 O44 93.9(5) . 3_666 ?
O46 K1 O45 77.7(5) . . ?
O46 K1 O50 66.9(6) . . ?
O50 K1 Ta3 77.3(4) . . ?
Eu1 O2 Cs1 102.2(3) . 1_655 ?
Se4 O2 Eu1 127.8(6) . . ?
Se4 O2 Cs1 99.6(4) . 1_655 ?
O12 O3 Ta5 67.4(8) . . ?
O8 O4 Ta6 67.5(6) . . ?
Se3 O5 Eu1 176.0(6) . . ?
O7 O6 Ta2 68.7(6) . . ?
Ta2 O7 Cs1 116.8(4) . 1_655 ?
O6 O7 Ta2 67.2(6) . . ?
O6 O7 Cs1 173.9(7) . 1_655 ?
Ta6 O8 Cs1 147.6(5) . 4_575 ?
O4 O8 Ta6 67.8(6) . . ?
O4 O8 Cs1 131.1(7) . 4_575 ?
Ta3 O9 K1 111.8(4) . . ?
O13 O9 Ta3 67.6(6) . . ?
O13 O9 K1 109.0(7) . . ?
Ta2 O10 Cs1 120.7(4) . 1_655 ?
Se4 O10 Ta2 124.0(6) . . ?
Se4 O10 Cs1 112.3(4) . 1_655 ?
O15 O11 Ta4 67.4(6) . . ?
Ta5 O12 K1 147.5(6) . 4_576 ?
O3 O12 Ta5 69.9(7) . . ?
O3 O12 K1 123.3(9) . 4_576 ?
O9 O13 Ta3 67.5(6) . . ?
Ta4 O14 Cs1 103.8(4) . . ?
Se2 O14 Ta4 129.5(6) . . ?
Se2 O14 Cs1 108.8(4) . . ?
Ta4 O15 Cs1 112.2(4) . . ?
O11 O15 Ta4 68.6(6) . . ?
O11 O15 Cs1 105.9(6) . . ?
Se3 O16 Ta4 136.2(6) . . ?
O19 O17 Ta1 67.7(6) . . ?
Se3 O18 Ta5 130.1(5) . . ?
O17 O19 Ta1 67.5(5) . . ?
Ta3 O20 Ta6 162.4(6) . . ?
Ta3 O21 K1 104.0(4) . . ?
Se1 O21 Ta3 126.4(5) . . ?
Se1 O21 K1 122.5(5) . . ?
Se2 O22 Ta6 125.1(6) . . ?
Ta1 O23 Ta4 163.5(5) . . ?
Se2 O24 Ta5 130.6(5) . . ?
Se4 O25 Ta1 122.2(5) . . ?
Se1 O26 Ta1 131.8(5) . . ?
Ta2 O27 Ta5 166.7(6) . . ?
Se1 O28 Ta2 130.8(5) . . ?
Ta5 O29 Ta6 110.0(5) . . ?
Ta6 O30 Ta4 106.5(4) . . ?
Ta3 O31 Ta1 108.4(4) . . ?
Ta4 O32 Ta5 146.3(5) . . ?
Ta4 O32 Ta6 108.3(4) . . ?
Ta6 O32 Ta5 100.1(4) . . ?
Ta3 O33 Ta2 107.9(4) . . ?
Ta1 O34 Ta2 143.8(5) . . ?
Ta1 O34 Ta3 106.7(4) . . ?
Ta3 O34 Ta2 106.0(4) . . ?
Eu1 O36 Cs1 159.7(5) . 4_676 ?
Eu1 O1 Cs1 109.7(4) . 1_655 ?
K1 O41 Cs1 147.5(5) 1_556 . ?
Eu1 O42 Cs1 97.5(4) . 1_655 ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy1_a_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 1893233'
loop_
_audit_author_name
_audit_author_address
'Dongdi Zhang'
;Henan University
China
;
_audit_update_record             
;
2022-04-25 deposited with the CCDC.	2022-05-24 downloaded from the CCDC.
;
_audit_creation_date             2021-08-23
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2016/6
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs K Lu O46 Se4 Ta6, 4(O)'
_chemical_formula_sum            'Cs K Lu O50 Se4 Ta6'
_chemical_formula_weight         2548.52
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Lu Lu -0.4720 5.8584 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.2537(9)
_cell_length_b                   27.308(2)
_cell_length_c                   13.9677(11)
_cell_angle_alpha                90
_cell_angle_beta                 114.1800(10)
_cell_angle_gamma                90
_cell_volume                     4263.9(6)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    3852
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.64
_cell_measurement_theta_min      2.35
_shelx_estimated_absorpt_T_max   0.161
_shelx_estimated_absorpt_T_min   0.090
_exptl_absorpt_coefficient_mu    22.111
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3686
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1443 before and 0.0554 after correction. The Ratio of minimum to maximum transmission is 0.4943. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.970
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4476
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.13
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0578
_diffrn_reflns_av_unetI/netI     0.0658
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            22026
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.098
_diffrn_reflns_theta_max         25.098
_diffrn_reflns_theta_min         1.491
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                5845
_reflns_number_total             7569
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         2.199
_refine_diff_density_min         -4.666
_refine_diff_density_rms         0.376
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.017
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7569
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0633
_refine_ls_R_factor_gt           0.0437
_refine_ls_restrained_S_all      1.017
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0404P)²+85.6174P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0968
_refine_ls_wR_factor_ref         0.1059
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28576(5) 0.54903(2) 0.55534(5) 0.01140(15) Uani 1 1 d . . . . .
Ta2 Ta 0.43790(5) 0.65824(2) 0.47007(5) 0.01139(15) Uani 1 1 d . . . . .
Ta3 Ta 0.17123(5) 0.60795(2) 0.32698(5) 0.01168(15) Uani 1 1 d . . . . .
Ta4 Ta 0.13567(5) 0.64093(2) 0.66356(5) 0.01173(15) Uani 1 1 d . . . . .
Ta5 Ta 0.28162(5) 0.75216(2) 0.57419(5) 0.01185(15) Uani 1 1 d . . . . .
Ta6 Ta 0.03031(5) 0.70166(2) 0.43658(5) 0.01322(15) Uani 1 1 d . . . . .
Lu1 Lu 0.68424(6) 0.64973(2) 0.98435(5) 0.01587(16) Uani 1 1 d . . . . .
Cs1 Cs -0.18168(14) 0.66374(7) 0.72064(15) 0.0691(5) Uani 1 1 d . . . . .
Se1 Se 0.41841(13) 0.53771(6) 0.38102(12) 0.0151(3) Uani 1 1 d . . . . .
Se2 Se 0.04738(13) 0.76027(6) 0.65836(13) 0.0158(3) Uani 1 1 d . . . . .
Se3 Se 0.37831(13) 0.71173(6) 0.82809(12) 0.0145(3) Uani 1 1 d . . . . .
Se4 Se 0.49249(14) 0.62470(6) 0.71394(13) 0.0174(4) Uani 1 1 d . . . . .
K1 K 0.2254(5) 0.5732(2) 0.0712(4) 0.0560(14) Uani 1 1 d . . . . .
O1 O 0.6200(9) 0.6151(4) 0.8188(9) 0.020(3) Uiso 1 1 d . . . . .
O2 O 0.3874(10) 0.8006(4) 0.5492(10) 0.028(3) Uiso 1 1 d . . . . .
O3 O -0.1411(9) 0.6925(4) 0.3402(9) 0.022(3) Uiso 1 1 d . . . . .
O4 O 0.5099(9) 0.6867(4) 0.8960(9) 0.019(2) Uiso 1 1 d . . . . .
O5 O 0.5039(10) 0.6927(4) 0.3816(9) 0.025(3) Uiso 1 1 d . . . . .
O6 O 0.5964(9) 0.6846(4) 0.4888(9) 0.023(3) Uiso 1 1 d . . . . .
O7 O -0.0823(10) 0.7373(4) 0.3141(9) 0.025(3) Uiso 1 1 d . . . . .
O8 O 0.0944(9) 0.6192(4) 0.1757(9) 0.020(2) Uiso 1 1 d . . . . .
O9 O 0.5459(9) 0.6368(4) 0.6206(9) 0.019(2) Uiso 1 1 d . . . . .
O10 O 0.1247(9) 0.6051(4) 0.7830(9) 0.021(3) Uiso 1 1 d . . . . .
O11 O 0.3150(11) 0.8212(5) 0.5995(10) 0.036(3) Uiso 1 1 d . . . . .
O12 O 0.0311(10) 0.5808(4) 0.2088(9) 0.026(3) Uiso 1 1 d . . . . .
O13 O 0.0689(9) 0.7032(4) 0.7083(9) 0.022(3) Uiso 1 1 d . . . . .
O14 O 0.0132(9) 0.6002(4) 0.6838(9) 0.020(3) Uiso 1 1 d . . . . .
O15 O 0.2970(9) 0.6596(4) 0.7826(9) 0.020(3) Uiso 1 1 d . . . . .
O16 O 0.2016(9) 0.4870(4) 0.5505(9) 0.023(3) Uiso 1 1 d . . . . .
O17 O 0.3986(9) 0.7283(4) 0.7177(8) 0.018(2) Uiso 1 1 d . . . . .
O18 O 0.3179(9) 0.4894(4) 0.6448(9) 0.021(3) Uiso 1 1 d . . . . .
O19 O 0.0877(9) 0.6581(4) 0.3610(8) 0.015(2) Uiso 1 1 d . . . . .
O20 O 0.2816(9) 0.5584(4) 0.2954(8) 0.018(2) Uiso 1 1 d . . . . .
O21 O -0.0281(8) 0.7487(4) 0.5285(8) 0.015(2) Uiso 1 1 d . . . . .
O22 O 0.2099(9) 0.5879(4) 0.6221(8) 0.017(2) Uiso 1 1 d . . . . .
O23 O 0.1853(9) 0.7756(4) 0.6664(9) 0.022(3) Uiso 1 1 d . . . . .
O24 O 0.4486(9) 0.5657(4) 0.6754(9) 0.020(3) Uiso 1 1 d . . . . .
O25 O 0.3822(9) 0.5172(4) 0.4815(8) 0.018(2) Uiso 1 1 d . . . . .
O26 O 0.3728(9) 0.7088(4) 0.5168(8) 0.015(2) Uiso 1 1 d . . . . .
O27 O 0.4942(8) 0.5905(4) 0.4280(8) 0.013(2) Uiso 1 1 d . . . . .
O28 O 0.1431(9) 0.7566(4) 0.4445(9) 0.020(2) Uiso 1 1 d . . . . .
O29 O -0.0081(9) 0.6450(4) 0.5184(8) 0.018(2) Uiso 1 1 d . . . . .
O30 O 0.1379(9) 0.5547(4) 0.4140(8) 0.018(2) Uiso 1 1 d . . . . .
O31 O 0.1804(8) 0.6896(4) 0.5756(8) 0.013(2) Uiso 1 1 d . . . . .
O32 O 0.2942(9) 0.6579(4) 0.3225(9) 0.019(2) Uiso 1 1 d . . . . .
O33 O 0.3097(8) 0.6092(3) 0.4778(8) 0.012(2) Uiso 1 1 d . . . . .
O34 O 0.5659(11) 0.6379(5) 1.0786(10) 0.036(3) Uiso 1 1 d . . . . .
O35 O 0.7024(11) 0.7260(4) 1.0794(10) 0.033(3) Uiso 1 1 d . . . . .
O36 O 0.8248(11) 0.6392(5) 1.1557(10) 0.035(3) Uiso 1 1 d . . . . .
O37 O 0.7564(11) 0.7086(5) 0.9084(11) 0.037(3) Uiso 1 1 d . . . . .
O40 O -0.2193(15) 0.6138(6) 0.4959(14) 0.067(5) Uiso 1 1 d . . . . .
O41 O 0.0493(13) 0.6454(5) 0.9261(13) 0.056(4) Uiso 1 1 d . . . . .
O42 O 0.8587(12) 0.6161(5) 0.9760(11) 0.045(4) Uiso 1 1 d . . . . .
O43 O 0.6716(12) 0.5670(5) 1.0058(11) 0.044(4) Uiso 1 1 d . . . . .
O45 O 0.3632(13) 0.5803(5) -0.0542(12) 0.052(4) Uiso 1 1 d . . . . .
O46 O 0.0933(15) 0.5151(6) -0.1073(14) 0.066(5) Uiso 1 1 d . . . . .
O50 O 0.139(2) 0.4703(9) 0.127(2) 0.133(9) Uiso 1 1 d . . . . .
O38 O -0.0465(12) 0.4987(5) 0.3454(11) 0.044(4) Uiso 1 1 d . . . . .
O39 O 0.6315(12) 0.7663(5) 0.7512(11) 0.043(4) Uiso 1 1 d . . . . .
O44 O 0.5838(12) 0.4984(5) 0.8479(11) 0.044(4) Uiso 1 1 d . . . . .
O47 O 0.3544(14) 0.4905(6) 0.8526(13) 0.065(5) Uiso 1 1 d . . . . .
O48 O 0.592(2) 0.6113(9) 1.271(2) 0.129(9) Uiso 1 1 d . . . . .
O49 O 0.273(2) 0.4411(10) 0.333(2) 0.141(10) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3264(9) . ?
Ta1 O16 1.969(11) . ?
Ta1 O18 1.991(11) . ?
Ta1 O22 1.889(11) . ?
Ta1 O24 2.064(10) . ?
Ta1 O25 2.052(11) . ?
Ta1 O30 2.067(10) . ?
Ta1 O33 2.055(10) . ?
Ta2 Ta3 3.3480(9) . ?
Ta2 Cs1 4.5427(18) 1_655 ?
Ta2 O5 1.971(12) . ?
Ta2 O6 1.985(11) . ?
Ta2 O9 2.058(11) . ?
Ta2 O26 1.842(10) . ?
Ta2 O27 2.139(10) . ?
Ta2 O32 2.092(11) . ?
Ta2 O33 2.100(10) . ?
Ta3 K1 4.006(5) . ?
Ta3 O8 1.953(11) . ?
Ta3 O12 1.976(11) . ?
Ta3 O19 1.884(10) . ?
Ta3 O20 2.085(10) . ?
Ta3 O30 2.041(11) . ?
Ta3 O32 2.052(10) . ?
Ta3 O33 2.095(10) . ?
Ta4 Ta6 3.3340(9) . ?
Ta4 Cs1 4.3227(18) . ?
Ta4 O10 1.985(11) . ?
Ta4 O13 2.090(11) . ?
Ta4 O14 1.979(11) . ?
Ta4 O15 2.059(11) . ?
Ta4 O22 1.922(10) . ?
Ta4 O29 2.074(10) . ?
Ta4 O31 2.032(10) . ?
Ta5 Ta6 3.1986(9) . ?
Ta5 O2 1.980(12) . ?
Ta5 O11 1.932(13) . ?
Ta5 O17 2.035(10) . ?
Ta5 O23 2.170(11) . ?
Ta5 O26 2.007(10) . ?
Ta5 O28 1.913(11) . ?
Ta5 O31 2.116(10) . ?
Ta6 O3 1.993(11) . ?
Ta6 O7 1.961(11) . ?
Ta6 O19 1.905(10) . ?
Ta6 O21 2.137(10) . ?
Ta6 O28 2.013(10) . ?
Ta6 O29 2.088(11) . ?
Ta6 O31 2.082(10) . ?
Lu1 Cs1 4.623(2) 1_655 ?
Lu1 O1 2.318(11) . ?
Lu1 O4 2.224(10) . ?
Lu1 O34 2.345(13) . ?
Lu1 O35 2.431(13) . ?
Lu1 O36 2.323(13) . ?
Lu1 O37 2.293(13) . ?
Lu1 O42 2.372(14) . ?
Lu1 O43 2.292(14) . ?
Cs1 O1 3.505(11) 1_455 ?
Cs1 O6 3.315(11) 1_455 ?
Cs1 O7 3.031(11) 4_576 ?
Cs1 O9 3.133(10) 1_455 ?
Cs1 O13 3.325(11) . ?
Cs1 O14 3.159(11) . ?
Cs1 O35 3.560(12) 4_475 ?
Cs1 O37 3.254(14) 1_455 ?
Cs1 O40 3.277(18) . ?
Cs1 O41 3.137(15) . ?
Cs1 O42 3.635(15) 1_455 ?
Cs1 O49 3.05(3) 3_566 ?
Se1 O20 1.708(10) . ?
Se1 O25 1.729(11) . ?
Se1 O27 1.694(10) . ?
Se2 O13 1.683(11) . ?
Se2 O21 1.695(10) . ?
Se2 O23 1.699(11) . ?
Se3 O4 1.647(10) . ?
Se3 O15 1.705(11) . ?
Se3 O17 1.720(11) . ?
Se4 O1 1.667(11) . ?
Se4 O9 1.714(11) . ?
Se4 O24 1.715(10) . ?
K1 O8 2.864(12) . ?
K1 O11 3.052(14) 4_575 ?
K1 O20 2.946(12) . ?
K1 O41 3.011(16) 1_554 ?
K1 O45 2.895(17) . ?
K1 O46 2.837(18) . ?
K1 O50 3.21(3) . ?
K1 O44 2.898(14) 3_666 ?
O2 O11 1.452(17) . ?
O3 O7 1.537(15) . ?
O5 O6 1.478(15) . ?
O8 O12 1.485(15) . ?
O10 O14 1.501(14) . ?
O16 O18 1.494(15) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 112.0(3) . . ?
O16 Ta1 O18 44.3(4) . . ?
O16 Ta1 O24 122.4(4) . . ?
O16 Ta1 O25 91.1(4) . . ?
O16 Ta1 O30 77.9(4) . . ?
O16 Ta1 O33 148.8(4) . . ?
O18 Ta1 Ta3 153.5(3) . . ?
O18 Ta1 O24 78.1(4) . . ?
O18 Ta1 O25 87.9(4) . . ?
O18 Ta1 O30 122.1(4) . . ?
O18 Ta1 O33 162.0(4) . . ?
O22 Ta1 Ta3 95.8(3) . . ?
O22 Ta1 O16 98.3(5) . . ?
O22 Ta1 O18 99.2(5) . . ?
O22 Ta1 O24 89.0(4) . . ?
O22 Ta1 O25 170.6(4) . . ?
O22 Ta1 O30 90.8(4) . . ?
O22 Ta1 O33 90.9(4) . . ?
O24 Ta1 Ta3 124.1(3) . . ?
O24 Ta1 O30 159.5(4) . . ?
O25 Ta1 Ta3 80.0(3) . . ?
O25 Ta1 O24 86.4(4) . . ?
O25 Ta1 O30 90.7(4) . . ?
O25 Ta1 O33 80.7(4) . . ?
O30 Ta1 Ta3 35.7(3) . . ?
O33 Ta1 Ta3 37.1(3) . . ?
O33 Ta1 O24 87.3(4) . . ?
O33 Ta1 O30 72.2(4) . . ?
Ta3 Ta2 Cs1 156.37(3) . 1_655 ?
O5 Ta2 Ta3 111.9(3) . . ?
O5 Ta2 Cs1 85.0(3) . 1_655 ?
O5 Ta2 O6 43.9(4) . . ?
O5 Ta2 O9 121.2(4) . . ?
O5 Ta2 O27 88.8(4) . . ?
O5 Ta2 O32 77.3(4) . . ?
O5 Ta2 O33 147.6(4) . . ?
O6 Ta2 Ta3 152.9(3) . . ?
O6 Ta2 Cs1 41.1(3) . 1_655 ?
O6 Ta2 O9 77.5(4) . . ?
O6 Ta2 O27 86.6(4) . . ?
O6 Ta2 O32 121.0(4) . . ?
O6 Ta2 O33 159.4(4) . . ?
O9 Ta2 Ta3 123.7(3) . . ?
O9 Ta2 Cs1 36.4(3) . 1_655 ?
O9 Ta2 O27 83.7(4) . . ?
O9 Ta2 O32 159.2(4) . . ?
O9 Ta2 O33 87.0(4) . . ?
O26 Ta2 Ta3 93.5(3) . . ?
O26 Ta2 Cs1 99.1(3) . 1_655 ?
O26 Ta2 O5 102.3(5) . . ?
O26 Ta2 O6 103.0(4) . . ?
O26 Ta2 O9 92.4(4) . . ?
O26 Ta2 O27 168.6(4) . . ?
O26 Ta2 O32 92.3(4) . . ?
O26 Ta2 O33 91.0(4) . . ?
O27 Ta2 Ta3 80.0(3) . . ?
O27 Ta2 Cs1 84.0(3) . 1_655 ?
O32 Ta2 Ta3 35.7(3) . . ?
O32 Ta2 Cs1 160.6(3) . 1_655 ?
O32 Ta2 O27 87.8(4) . . ?
O32 Ta2 O33 72.7(4) . . ?
O33 Ta2 Ta3 37.0(3) . . ?
O33 Ta2 Cs1 122.3(3) . 1_655 ?
O33 Ta2 O27 78.2(4) . . ?
Ta1 Ta3 Ta2 72.586(19) . . ?
Ta1 Ta3 K1 125.58(7) . . ?
Ta2 Ta3 K1 98.74(8) . . ?
O8 Ta3 Ta1 160.1(3) . . ?
O8 Ta3 Ta2 120.1(3) . . ?
O8 Ta3 K1 41.8(3) . . ?
O8 Ta3 O12 44.4(4) . . ?
O8 Ta3 O20 86.6(4) . . ?
O8 Ta3 O30 129.1(4) . . ?
O8 Ta3 O32 84.1(4) . . ?
O8 Ta3 O33 156.6(4) . . ?
O12 Ta3 Ta1 120.0(3) . . ?
O12 Ta3 Ta2 162.7(4) . . ?
O12 Ta3 K1 64.6(4) . . ?
O12 Ta3 O20 89.8(4) . . ?
O12 Ta3 O30 85.0(4) . . ?
O12 Ta3 O32 128.5(5) . . ?
O12 Ta3 O33 156.3(4) . . ?
O19 Ta3 Ta1 99.8(3) . . ?
O19 Ta3 Ta2 92.8(3) . . ?
O19 Ta3 K1 134.6(3) . . ?
O19 Ta3 O8 95.0(4) . . ?
O19 Ta3 O12 96.2(4) . . ?
O19 Ta3 O20 172.9(4) . . ?
O19 Ta3 O30 96.1(4) . . ?
O19 Ta3 O32 90.3(4) . . ?
O19 Ta3 O33 92.0(4) . . ?
O20 Ta3 Ta1 80.4(3) . . ?
O20 Ta3 Ta2 80.4(3) . . ?
O20 Ta3 K1 45.5(3) . . ?
O20 Ta3 O33 84.0(4) . . ?
O30 Ta3 Ta1 36.2(3) . . ?
O30 Ta3 Ta2 108.7(3) . . ?
O30 Ta3 K1 120.6(3) . . ?
O30 Ta3 O20 88.2(4) . . ?
O30 Ta3 O32 145.1(4) . . ?
O30 Ta3 O33 72.0(4) . . ?
O32 Ta3 Ta1 108.9(3) . . ?
O32 Ta3 Ta2 36.5(3) . . ?
O32 Ta3 K1 74.8(3) . . ?
O32 Ta3 O20 83.0(4) . . ?
O32 Ta3 O33 73.6(4) . . ?
O33 Ta3 Ta1 36.3(3) . . ?
O33 Ta3 Ta2 37.1(3) . . ?
O33 Ta3 K1 122.6(3) . . ?
Ta6 Ta4 Cs1 94.39(3) . . ?
O10 Ta4 Ta6 155.7(3) . . ?
O10 Ta4 Cs1 62.6(3) . . ?
O10 Ta4 O13 88.9(4) . . ?
O10 Ta4 O15 79.4(4) . . ?
O10 Ta4 O29 121.7(4) . . ?
O10 Ta4 O31 163.4(4) . . ?
O13 Ta4 Ta6 80.4(3) . . ?
O13 Ta4 Cs1 48.4(3) . . ?
O14 Ta4 Ta6 113.2(3) . . ?
O14 Ta4 Cs1 42.5(3) . . ?
O14 Ta4 O10 44.5(4) . . ?
O14 Ta4 O13 90.1(4) . . ?
O14 Ta4 O15 123.9(4) . . ?
O14 Ta4 O29 77.3(4) . . ?
O14 Ta4 O31 149.5(4) . . ?
O15 Ta4 Ta6 121.0(3) . . ?
O15 Ta4 Cs1 117.0(3) . . ?
O15 Ta4 O13 85.5(4) . . ?
O15 Ta4 O29 157.9(4) . . ?
O22 Ta4 Ta6 97.7(3) . . ?
O22 Ta4 Cs1 137.5(3) . . ?
O22 Ta4 O10 94.9(4) . . ?
O22 Ta4 O13 174.1(4) . . ?
O22 Ta4 O14 95.8(4) . . ?
O22 Ta4 O15 90.8(4) . . ?
O22 Ta4 O29 93.6(4) . . ?
O22 Ta4 O31 91.9(4) . . ?
O29 Ta4 Ta6 36.9(3) . . ?
O29 Ta4 Cs1 72.8(3) . . ?
O29 Ta4 O13 88.2(4) . . ?
O31 Ta4 Ta6 36.4(3) . . ?
O31 Ta4 Cs1 120.2(3) . . ?
O31 Ta4 O13 83.3(4) . . ?
O31 Ta4 O15 85.4(4) . . ?
O31 Ta4 O29 72.8(4) . . ?
O2 Ta5 Ta6 136.1(3) . . ?
O2 Ta5 O17 98.0(4) . . ?
O2 Ta5 O23 117.5(4) . . ?
O2 Ta5 O26 79.2(4) . . ?
O2 Ta5 O31 165.8(4) . . ?
O11 Ta5 Ta6 127.6(4) . . ?
O11 Ta5 O2 43.5(5) . . ?
O11 Ta5 O17 96.9(5) . . ?
O11 Ta5 O23 74.3(5) . . ?
O11 Ta5 O26 122.6(5) . . ?
O11 Ta5 O31 150.2(5) . . ?
O17 Ta5 Ta6 124.8(3) . . ?
O17 Ta5 O23 81.1(4) . . ?
O17 Ta5 O31 85.0(4) . . ?
O23 Ta5 Ta6 81.9(3) . . ?
O26 Ta5 Ta6 93.5(3) . . ?
O26 Ta5 O17 85.5(4) . . ?
O26 Ta5 O23 159.8(4) . . ?
O26 Ta5 O31 87.2(4) . . ?
O28 Ta5 Ta6 36.5(3) . . ?
O28 Ta5 O2 100.5(5) . . ?
O28 Ta5 O11 98.6(5) . . ?
O28 Ta5 O17 161.3(4) . . ?
O28 Ta5 O23 93.2(4) . . ?
O28 Ta5 O26 94.7(4) . . ?
O28 Ta5 O31 76.4(4) . . ?
O31 Ta5 Ta6 40.0(3) . . ?
O31 Ta5 O23 76.7(4) . . ?
Ta5 Ta6 Ta4 74.96(2) . . ?
O3 Ta6 Ta4 118.1(3) . . ?
O3 Ta6 Ta5 161.6(3) . . ?
O3 Ta6 O21 87.8(4) . . ?
O3 Ta6 O28 129.8(4) . . ?
O3 Ta6 O29 82.3(4) . . ?
O3 Ta6 O31 153.4(4) . . ?
O7 Ta6 Ta4 159.5(3) . . ?
O7 Ta6 Ta5 118.1(3) . . ?
O7 Ta6 O3 45.7(4) . . ?
O7 Ta6 O21 86.3(4) . . ?
O7 Ta6 O28 84.2(4) . . ?
O7 Ta6 O29 127.5(4) . . ?
O7 Ta6 O31 158.3(4) . . ?
O19 Ta6 Ta4 97.5(3) . . ?
O19 Ta6 Ta5 96.8(3) . . ?
O19 Ta6 O3 94.2(4) . . ?
O19 Ta6 O7 96.5(5) . . ?
O19 Ta6 O21 177.1(4) . . ?
O19 Ta6 O28 95.4(4) . . ?
O19 Ta6 O29 93.3(4) . . ?
O19 Ta6 O31 91.9(4) . . ?
O21 Ta6 Ta4 79.8(3) . . ?
O21 Ta6 Ta5 81.8(3) . . ?
O28 Ta6 Ta4 109.2(3) . . ?
O28 Ta6 Ta5 34.4(3) . . ?
O28 Ta6 O21 84.8(4) . . ?
O28 Ta6 O29 145.7(4) . . ?
O28 Ta6 O31 75.1(4) . . ?
O29 Ta6 Ta4 36.6(3) . . ?
O29 Ta6 Ta5 111.6(3) . . ?
O29 Ta6 O21 84.9(4) . . ?
O31 Ta6 Ta4 35.4(3) . . ?
O31 Ta6 Ta5 40.7(3) . . ?
O31 Ta6 O21 85.4(4) . . ?
O31 Ta6 O29 71.6(4) . . ?
O1 Lu1 Cs1 47.6(3) . 1_655 ?
O1 Lu1 O34 117.9(4) . . ?
O1 Lu1 O35 144.4(4) . . ?
O1 Lu1 O36 141.5(4) . . ?
O1 Lu1 O42 74.8(4) . . ?
O4 Lu1 Cs1 95.4(3) . 1_655 ?
O4 Lu1 O1 77.0(4) . . ?
O4 Lu1 O34 72.5(4) . . ?
O4 Lu1 O35 76.5(4) . . ?
O4 Lu1 O36 140.0(4) . . ?
O4 Lu1 O37 83.6(4) . . ?
O4 Lu1 O42 145.9(4) . . ?
O4 Lu1 O43 114.8(4) . . ?
O34 Lu1 Cs1 164.1(3) . 1_655 ?
O34 Lu1 O35 75.5(4) . . ?
O34 Lu1 O42 138.7(5) . . ?
O35 Lu1 Cs1 112.4(3) . 1_655 ?
O36 Lu1 Cs1 118.4(3) . 1_655 ?
O36 Lu1 O34 76.9(4) . . ?
O36 Lu1 O35 71.4(4) . . ?
O36 Lu1 O42 72.5(5) . . ?
O37 Lu1 Cs1 40.8(3) . 1_655 ?
O37 Lu1 O1 82.1(4) . . ?
O37 Lu1 O34 143.1(4) . . ?
O37 Lu1 O35 71.7(5) . . ?
O37 Lu1 O36 107.4(5) . . ?
O37 Lu1 O42 73.9(5) . . ?
O42 Lu1 Cs1 51.1(3) . 1_655 ?
O42 Lu1 O35 118.4(4) . . ?
O43 Lu1 Cs1 104.5(4) . 1_655 ?
O43 Lu1 O1 73.4(4) . . ?
O43 Lu1 O34 72.6(5) . . ?
O43 Lu1 O35 140.2(5) . . ?
O43 Lu1 O36 78.7(5) . . ?
O43 Lu1 O37 144.2(5) . . ?
O43 Lu1 O42 74.7(5) . . ?
O1 Cs1 O35 110.8(3) 1_455 4_475 ?
O1 Cs1 O42 47.0(3) 1_455 1_455 ?
O6 Cs1 O1 91.4(3) 1_455 1_455 ?
O6 Cs1 O13 107.4(3) 1_455 . ?
O6 Cs1 O35 48.1(3) 1_455 4_475 ?
O6 Cs1 O42 138.4(3) 1_455 1_455 ?
O7 Cs1 O1 113.0(3) 4_576 1_455 ?
O7 Cs1 O6 107.0(3) 4_576 1_455 ?
O7 Cs1 O9 124.6(3) 4_576 1_455 ?
O7 Cs1 O13 61.1(3) 4_576 . ?
O7 Cs1 O14 111.2(3) 4_576 . ?
O7 Cs1 O35 58.9(3) 4_576 4_475 ?
O7 Cs1 O37 60.2(3) 4_576 1_455 ?
O7 Cs1 O40 131.1(4) 4_576 . ?
O7 Cs1 O41 72.3(3) 4_576 . ?
O7 Cs1 O42 91.5(3) 4_576 1_455 ?
O7 Cs1 O49 169.8(6) 4_576 3_566 ?
O9 Cs1 O1 45.8(3) 1_455 1_455 ?
O9 Cs1 O6 46.1(3) 1_455 1_455 ?
O9 Cs1 O13 153.0(3) 1_455 . ?
O9 Cs1 O14 122.5(3) 1_455 . ?
O9 Cs1 O35 80.9(3) 1_455 4_475 ?
O9 Cs1 O37 83.7(3) 1_455 1_455 ?
O9 Cs1 O40 76.6(4) 1_455 . ?
O9 Cs1 O41 140.2(4) 1_455 . ?
O9 Cs1 O42 92.6(3) 1_455 1_455 ?
O13 Cs1 O1 161.2(3) . 1_455 ?
O13 Cs1 O35 82.2(3) . 4_475 ?
O13 Cs1 O42 114.2(3) . 1_455 ?
O14 Cs1 O1 123.2(3) . 1_455 ?
O14 Cs1 O6 107.9(3) . 1_455 ?
O14 Cs1 O13 52.7(3) . . ?
O14 Cs1 O35 122.0(3) . 4_475 ?
O14 Cs1 O37 141.2(3) . 1_455 ?
O14 Cs1 O40 55.6(3) . . ?
O14 Cs1 O42 98.9(3) . 1_455 ?
O35 Cs1 O42 135.2(3) 4_475 1_455 ?
O37 Cs1 O1 53.1(3) 1_455 1_455 ?
O37 Cs1 O6 110.7(3) 1_455 1_455 ?
O37 Cs1 O13 116.4(3) 1_455 . ?
O37 Cs1 O35 87.5(3) 1_455 4_475 ?
O37 Cs1 O40 160.2(4) 1_455 . ?
O37 Cs1 O42 47.7(3) 1_455 1_455 ?
O40 Cs1 O1 111.7(3) . 1_455 ?
O40 Cs1 O6 53.0(3) . 1_455 ?
O40 Cs1 O13 81.7(4) . . ?
O40 Cs1 O35 87.3(4) . 4_475 ?
O40 Cs1 O42 134.5(4) . 1_455 ?
O41 Cs1 O1 95.3(3) . 1_455 ?
O41 Cs1 O6 173.0(4) . 1_455 ?
O41 Cs1 O13 66.0(4) . . ?
O41 Cs1 O14 66.6(4) . . ?
O41 Cs1 O35 130.3(3) . 4_475 ?
O41 Cs1 O37 75.1(4) . 1_455 ?
O41 Cs1 O40 122.0(4) . . ?
O41 Cs1 O42 48.4(4) . 1_455 ?
O49 Cs1 O1 59.9(6) 3_566 1_455 ?
O49 Cs1 O6 81.3(5) 3_566 1_455 ?
O49 Cs1 O9 56.9(5) 3_566 1_455 ?
O49 Cs1 O13 122.9(6) 3_566 . ?
O49 Cs1 O14 70.7(6) 3_566 . ?
O49 Cs1 O35 129.3(6) 3_566 4_475 ?
O49 Cs1 O37 111.7(6) 3_566 1_455 ?
O49 Cs1 O40 58.6(6) 3_566 . ?
O49 Cs1 O41 100.3(6) 3_566 . ?
O49 Cs1 O42 78.3(6) 3_566 1_455 ?
O20 Se1 O25 99.8(5) . . ?
O27 Se1 O20 102.4(5) . . ?
O27 Se1 O25 104.1(5) . . ?
O13 Se2 Cs1 48.5(4) . . ?
O13 Se2 O21 101.3(5) . . ?
O13 Se2 O23 102.6(5) . . ?
O21 Se2 Cs1 89.3(3) . . ?
O21 Se2 O23 102.0(5) . . ?
O23 Se2 Cs1 150.9(4) . . ?
O4 Se3 O15 98.8(5) . . ?
O4 Se3 O17 99.1(5) . . ?
O15 Se3 O17 99.4(5) . . ?
O1 Se4 Cs1 57.8(4) . 1_655 ?
O1 Se4 O9 100.7(5) . . ?
O1 Se4 O24 100.8(5) . . ?
O9 Se4 Cs1 45.1(3) . 1_655 ?
O9 Se4 O24 96.4(5) . . ?
O24 Se4 Cs1 115.4(4) . 1_655 ?
O8 K1 Ta3 27.0(2) . . ?
O8 K1 O11 76.6(3) . 4_575 ?
O8 K1 O20 56.9(3) . . ?
O8 K1 O41 70.1(4) . 1_554 ?
O8 K1 O45 150.1(4) . . ?
O8 K1 O50 87.1(6) . . ?
O8 K1 O44 128.9(4) . 3_666 ?
O11 K1 Ta3 81.0(3) 4_575 . ?
O11 K1 O50 158.8(6) 4_575 . ?
O20 K1 Ta3 30.3(2) . . ?
O20 K1 O11 94.4(4) . 4_575 ?
O20 K1 O41 126.6(4) . 1_554 ?
O20 K1 O50 65.0(5) . . ?
O41 K1 Ta3 96.3(3) 1_554 . ?
O41 K1 O11 65.8(4) 1_554 4_575 ?
O41 K1 O50 121.4(6) 1_554 . ?
O45 K1 Ta3 151.0(3) . . ?
O45 K1 O11 75.4(4) . 4_575 ?
O45 K1 O20 135.4(4) . . ?
O45 K1 O41 89.1(5) . 1_554 ?
O45 K1 O50 122.5(6) . . ?
O45 K1 O44 72.7(4) . 3_666 ?
O46 K1 Ta3 132.3(4) . . ?
O46 K1 O8 117.1(4) . . ?
O46 K1 O11 133.4(5) . 4_575 ?
O46 K1 O20 131.2(4) . . ?
O46 K1 O41 77.4(5) . 1_554 ?
O46 K1 O45 76.7(5) . . ?
O46 K1 O50 66.3(6) . . ?
O46 K1 O44 92.5(5) . 3_666 ?
O50 K1 Ta3 78.4(5) . . ?
O44 K1 Ta3 102.3(3) 3_666 . ?
O44 K1 O11 113.3(4) 3_666 4_575 ?
O44 K1 O20 72.1(4) 3_666 . ?
O44 K1 O41 161.0(5) 3_666 1_554 ?
O44 K1 O50 66.9(5) 3_666 . ?
Lu1 O1 Cs1 103.2(3) . 1_655 ?
Se4 O1 Lu1 128.7(6) . . ?
Se4 O1 Cs1 98.4(5) . 1_655 ?
O11 O2 Ta5 66.5(7) . . ?
O7 O3 Ta6 66.0(6) . . ?
Se3 O4 Lu1 177.4(6) . . ?
O6 O5 Ta2 68.6(6) . . ?
Ta2 O6 Cs1 115.7(5) . 1_655 ?
O5 O6 Ta2 67.5(6) . . ?
O5 O6 Cs1 175.5(8) . 1_655 ?
Ta6 O7 Cs1 146.5(5) . 4_575 ?
O3 O7 Ta6 68.2(6) . . ?
O3 O7 Cs1 131.8(7) . 4_575 ?
Ta3 O8 K1 111.1(4) . . ?
O12 O8 Ta3 68.6(6) . . ?
O12 O8 K1 108.8(7) . . ?
Ta2 O9 Cs1 120.7(4) . 1_655 ?
Se4 O9 Ta2 123.1(6) . . ?
Se4 O9 Cs1 112.0(5) . 1_655 ?
O14 O10 Ta4 67.5(6) . . ?
Ta5 O11 K1 149.3(6) . 4_576 ?
O2 O11 Ta5 70.0(7) . . ?
O2 O11 K1 124.3(8) . 4_576 ?
O8 O12 Ta3 67.0(6) . . ?
Ta4 O13 Cs1 103.6(4) . . ?
Se2 O13 Ta4 130.1(6) . . ?
Se2 O13 Cs1 109.3(5) . . ?
Ta4 O14 Cs1 112.5(4) . . ?
O10 O14 Ta4 68.0(6) . . ?
O10 O14 Cs1 105.3(7) . . ?
Se3 O15 Ta4 136.8(6) . . ?
O18 O16 Ta1 68.6(6) . . ?
Se3 O17 Ta5 131.7(6) . . ?
O16 O18 Ta1 67.1(6) . . ?
Ta3 O19 Ta6 162.8(6) . . ?
Ta3 O20 K1 104.2(4) . . ?
Se1 O20 Ta3 127.0(6) . . ?
Se1 O20 K1 121.7(5) . . ?
Se2 O21 Ta6 125.8(5) . . ?
Ta1 O22 Ta4 164.1(6) . . ?
Se2 O23 Ta5 131.0(6) . . ?
Se4 O24 Ta1 122.5(6) . . ?
Se1 O25 Ta1 131.5(6) . . ?
Ta2 O26 Ta5 167.6(6) . . ?
Se1 O27 Ta2 130.9(5) . . ?
Ta5 O28 Ta6 109.1(5) . . ?
Ta4 O29 Ta6 106.4(4) . . ?
Ta3 O30 Ta1 108.1(5) . . ?
Ta4 O31 Ta5 146.9(5) . . ?
Ta4 O31 Ta6 108.3(4) . . ?
Ta6 O31 Ta5 99.3(4) . . ?
Ta3 O32 Ta2 107.8(5) . . ?
Ta1 O33 Ta2 143.9(5) . . ?
Ta1 O33 Ta3 106.5(4) . . ?
Ta3 O33 Ta2 105.9(4) . . ?
Lu1 O35 Cs1 162.5(5) . 4_676 ?
Lu1 O37 Cs1 111.7(5) . 1_655 ?
K1 O41 Cs1 148.1(6) 1_556 . ?
Lu1 O42 Cs1 98.4(4) . 1_655 ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy1_a_CCDC2
_database_code_depnum_ccdc_archive 'CCDC 2168599'
loop_
_audit_author_name
_audit_author_address
'Dongdi Zhang'
;Henan University
China
;
_audit_update_record             
;
2022-04-25 deposited with the CCDC.	2022-05-24 downloaded from the CCDC.
;
_audit_creation_date             2021-08-04
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2016/6
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs Gd K O46 Se4 Ta6, 4(O)'
_chemical_formula_sum            'Cs Gd K O50 Se4 Ta6'
_chemical_formula_weight         2530.80
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.3307(5)
_cell_length_b                   27.2604(11)
_cell_length_c                   14.0160(6)
_cell_angle_alpha                90
_cell_angle_beta                 113.8540(10)
_cell_angle_gamma                90
_cell_volume                     4308.9(3)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    6757
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.33
_cell_measurement_theta_min      2.18
_shelx_estimated_absorpt_T_max   0.170
_shelx_estimated_absorpt_T_min   0.052
_exptl_absorpt_coefficient_mu    21.128
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.2782
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1374 before and 0.0501 after correction.
The Ratio of minimum to maximum transmission is 0.3731.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.901
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4448
_exptl_crystal_size_max          0.34
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.13
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0422
_diffrn_reflns_av_unetI/netI     0.0478
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22215
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.755
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6417
_reflns_number_total             7652
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         1.767
_refine_diff_density_min         -4.924
_refine_diff_density_rms         0.327
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7652
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0493
_refine_ls_R_factor_gt           0.0388
_refine_ls_restrained_S_all      1.023
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0377P)²+112.6546P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0910
_refine_ls_wR_factor_ref         0.0963
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28562(4) 0.54854(2) 0.55513(4) 0.01087(12) Uani 1 1 d . . . . .
Ta2 Ta 0.43741(4) 0.65792(2) 0.47008(4) 0.01103(12) Uani 1 1 d . . . . .
Ta3 Ta 0.17262(4) 0.60777(2) 0.32837(4) 0.01136(12) Uani 1 1 d . . . . .
Ta4 Ta 0.13710(4) 0.64072(2) 0.66434(4) 0.01110(12) Uani 1 1 d . . . . .
Ta5 Ta 0.28293(4) 0.75200(2) 0.57518(4) 0.01180(12) Uani 1 1 d . . . . .
Ta6 Ta 0.03282(4) 0.70166(2) 0.43858(4) 0.01374(13) Uani 1 1 d . . . . .
Gd1 Gd 0.68537(6) 0.64917(2) 0.98594(5) 0.01601(15) Uani 1 1 d . . . . .
Se1 Se 0.41747(11) 0.53713(5) 0.38111(9) 0.0152(3) Uani 1 1 d . . . . .
Se2 Se 0.05053(11) 0.76047(5) 0.65979(10) 0.0159(3) Uani 1 1 d . . . . .
Se3 Se 0.37663(11) 0.71176(5) 0.82756(9) 0.0135(3) Uani 1 1 d . . . . .
Se4 Se 0.49189(11) 0.62373(5) 0.71303(9) 0.0162(3) Uani 1 1 d . . . . .
Cs1 Cs -0.18134(12) 0.66335(6) 0.72012(12) 0.0661(4) Uani 1 1 d . . . . .
K1 K 0.2256(4) 0.57410(18) 0.0721(4) 0.0599(12) Uani 1 1 d . . . . .
O1 O 0.6180(8) 0.6137(3) 0.8148(7) 0.023(2) Uiso 1 1 d . . . . .
O2 O 0.3862(10) 0.8002(4) 0.5489(8) 0.036(3) Uiso 1 1 d . . . . .
O3 O -0.1361(9) 0.6941(4) 0.3430(8) 0.028(2) Uiso 1 1 d . . . . .
O4 O 0.5066(8) 0.6872(3) 0.8964(7) 0.021(2) Uiso 1 1 d . . . . .
O5 O 0.5028(8) 0.6928(3) 0.3818(7) 0.020(2) Uiso 1 1 d . . . . .
O6 O 0.5952(8) 0.6847(3) 0.4885(7) 0.020(2) Uiso 1 1 d . . . . .
O7 O -0.0783(9) 0.7378(4) 0.3166(7) 0.027(2) Uiso 1 1 d . . . . .
O8 O 0.0973(8) 0.6196(3) 0.1771(7) 0.022(2) Uiso 1 1 d . . . . .
O9 O 0.5449(8) 0.6374(4) 0.6197(7) 0.024(2) Uiso 1 1 d . . . . .
O10 O 0.1264(8) 0.6043(3) 0.7841(7) 0.020(2) Uiso 1 1 d . . . . .
O11 O 0.3170(10) 0.8222(4) 0.6030(9) 0.041(3) Uiso 1 1 d . . . . .
O12 O 0.0331(8) 0.5796(3) 0.2121(7) 0.021(2) Uiso 1 1 d . . . . .
O13 O 0.0702(8) 0.7028(3) 0.7094(7) 0.018(2) Uiso 1 1 d . . . . .
O14 O 0.0162(8) 0.5995(3) 0.6864(7) 0.021(2) Uiso 1 1 d . . . . .
O15 O 0.2957(8) 0.6591(3) 0.7826(7) 0.0177(19) Uiso 1 1 d . . . . .
O16 O 0.2016(8) 0.4863(4) 0.5513(7) 0.024(2) Uiso 1 1 d . . . . .
O17 O 0.3990(7) 0.7284(3) 0.7183(6) 0.0154(19) Uiso 1 1 d . . . . .
O18 O 0.3176(8) 0.4884(3) 0.6440(7) 0.022(2) Uiso 1 1 d . . . . .
O19 O 0.0889(8) 0.6574(3) 0.3645(6) 0.0154(19) Uiso 1 1 d . . . . .
O20 O 0.2812(7) 0.5576(3) 0.2960(6) 0.0149(19) Uiso 1 1 d . . . . .
O21 O -0.0247(8) 0.7491(3) 0.5302(7) 0.0167(19) Uiso 1 1 d . . . . .
O22 O 0.2096(8) 0.5878(3) 0.6217(6) 0.0164(19) Uiso 1 1 d . . . . .
O23 O 0.1869(8) 0.7761(3) 0.6665(7) 0.019(2) Uiso 1 1 d . . . . .
O24 O 0.4466(8) 0.5648(3) 0.6744(7) 0.0179(19) Uiso 1 1 d . . . . .
O25 O 0.3835(7) 0.5168(3) 0.4816(6) 0.0153(19) Uiso 1 1 d . . . . .
O26 O 0.3721(7) 0.7085(3) 0.5164(6) 0.0155(19) Uiso 1 1 d . . . . .
O27 O 0.4916(8) 0.5901(3) 0.4255(7) 0.019(2) Uiso 1 1 d . . . . .
O28 O 0.1445(8) 0.7566(3) 0.4462(7) 0.021(2) Uiso 1 1 d . . . . .
O29 O -0.0054(8) 0.6453(3) 0.5207(7) 0.019(2) Uiso 1 1 d . . . . .
O30 O 0.1385(8) 0.5541(3) 0.4132(7) 0.019(2) Uiso 1 1 d . . . . .
O31 O 0.1813(7) 0.6898(3) 0.5764(6) 0.0128(18) Uiso 1 1 d . . . . .
O32 O 0.2938(8) 0.6577(3) 0.3230(7) 0.019(2) Uiso 1 1 d . . . . .
O33 O 0.3099(7) 0.6090(3) 0.4781(6) 0.0117(18) Uiso 1 1 d . . . . .
O34 O 0.5637(10) 0.6365(4) 1.0828(8) 0.035(3) Uiso 1 1 d . . . . .
O35 O 0.7008(10) 0.7277(4) 1.0833(8) 0.037(3) Uiso 1 1 d . . . . .
O36 O 0.8317(10) 0.6392(4) 1.1627(8) 0.036(3) Uiso 1 1 d . . . . .
O37 O 0.7593(11) 0.7109(4) 0.9071(9) 0.044(3) Uiso 1 1 d . . . . .
O38 O -0.0462(10) 0.5000(4) 0.3458(9) 0.040(3) Uiso 1 1 d . . . . .
O39 O 0.6283(10) 0.7684(4) 0.7520(9) 0.044(3) Uiso 1 1 d . . . . .
O40 O -0.2145(12) 0.6138(5) 0.4992(11) 0.061(4) Uiso 1 1 d . . . . .
O41 O 0.0521(12) 0.6449(5) 0.9275(10) 0.056(4) Uiso 1 1 d . . . . .
O42 O 0.8645(11) 0.6145(5) 0.9761(10) 0.051(3) Uiso 1 1 d . . . . .
O43 O 0.6783(11) 0.5638(5) 1.0086(9) 0.045(3) Uiso 1 1 d . . . . .
O44 O 0.5820(12) 0.4966(5) 0.8442(10) 0.053(3) Uiso 1 1 d . . . . .
O45 O 0.3619(12) 0.5819(5) -0.0550(10) 0.058(4) Uiso 1 1 d . . . . .
O46 O 0.0957(13) 0.5151(6) -0.1032(12) 0.068(4) Uiso 1 1 d . . . . .
O47 O 0.3573(13) 0.4929(6) 0.8519(11) 0.068(4) Uiso 1 1 d . . . . .
O48 O 0.6045(17) 0.6133(7) 1.2809(15) 0.097(6) Uiso 1 1 d . . . . .
O49 O 0.273(3) 0.4414(11) 0.330(2) 0.166(11) Uiso 1 1 d . . . . .
O50 O 0.140(2) 0.4725(9) 0.1290(18) 0.128(8) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3270(7) . ?
Ta1 O16 1.978(10) . ?
Ta1 O18 2.000(9) . ?
Ta1 O22 1.898(9) . ?
Ta1 O24 2.061(9) . ?
Ta1 O25 2.067(8) . ?
Ta1 O30 2.086(9) . ?
Ta1 O33 2.058(8) . ?
Ta2 Ta3 3.3511(7) . ?
Ta2 O5 1.972(9) . ?
Ta2 O6 1.995(9) . ?
Ta2 O9 2.054(9) . ?
Ta2 O26 1.842(9) . ?
Ta2 O27 2.144(9) . ?
Ta2 O32 2.105(9) . ?
Ta2 O33 2.099(8) . ?
Ta3 K1 4.009(4) . ?
Ta3 O8 1.967(9) . ?
Ta3 O12 1.984(9) . ?
Ta3 O19 1.890(9) . ?
Ta3 O20 2.089(8) . ?
Ta3 O30 2.033(9) . ?
Ta3 O32 2.045(9) . ?
Ta3 O33 2.097(8) . ?
Ta4 Ta6 3.3369(7) . ?
Ta4 Cs1 4.3466(15) . ?
Ta4 O10 1.999(9) . ?
Ta4 O13 2.089(9) . ?
Ta4 O14 1.988(9) . ?
Ta4 O15 2.050(9) . ?
Ta4 O22 1.915(9) . ?
Ta4 O29 2.072(9) . ?
Ta4 O31 2.036(8) . ?
Ta5 Ta6 3.2070(7) . ?
Ta5 O2 1.965(11) . ?
Ta5 O11 1.964(12) . ?
Ta5 O17 2.040(8) . ?
Ta5 O23 2.167(9) . ?
Ta5 O26 2.006(9) . ?
Ta5 O28 1.924(9) . ?
Ta5 O31 2.113(8) . ?
Ta6 O3 1.979(10) . ?
Ta6 O7 1.969(10) . ?
Ta6 O19 1.896(8) . ?
Ta6 O21 2.136(9) . ?
Ta6 O28 2.007(9) . ?
Ta6 O29 2.084(9) . ?
Ta6 O31 2.081(8) . ?
Gd1 Cs1 4.6567(16) 1_655 ?
Gd1 O1 2.401(9) . ?
Gd1 O4 2.296(9) . ?
Gd1 O34 2.420(11) . ?
Gd1 O35 2.504(11) . ?
Gd1 O36 2.419(11) . ?
Gd1 O37 2.387(12) . ?
Gd1 O42 2.457(13) . ?
Gd1 O43 2.355(12) . ?
Se1 O20 1.713(8) . ?
Se1 O25 1.715(8) . ?
Se1 O27 1.687(9) . ?
Se2 Cs1 4.225(2) . ?
Se2 O13 1.697(9) . ?
Se2 O21 1.701(8) . ?
Se2 O23 1.700(9) . ?
Se3 O4 1.643(9) . ?
Se3 O15 1.715(9) . ?
Se3 O17 1.723(8) . ?
Se4 Cs1 4.1337(19) 1_655 ?
Se4 O1 1.654(9) . ?
Se4 O9 1.723(9) . ?
Se4 O24 1.715(9) . ?
Cs1 O1 3.517(9) 1_455 ?
Cs1 O6 3.353(9) 1_455 ?
Cs1 O7 3.052(10) 4_576 ?
Cs1 O9 3.168(10) 1_455 ?
Cs1 O13 3.343(9) . ?
Cs1 O14 3.181(9) . ?
Cs1 O35 3.515(11) 4_475 ?
Cs1 O37 3.261(12) 1_455 ?
Cs1 O40 3.248(14) . ?
Cs1 O41 3.197(14) . ?
Cs1 O42 3.650(13) 1_455 ?
Cs1 O49 3.05(3) 3_566 ?
K1 O8 2.845(10) . ?
K1 O11 3.010(13) 4_575 ?
K1 O20 2.964(9) . ?
K1 O41 2.983(14) 1_554 ?
K1 O44 2.910(14) 3_666 ?
K1 O45 2.909(15) . ?
K1 O46 2.829(16) . ?
K1 O50 3.18(2) . ?
O2 O11 1.478(15) . ?
O3 O7 1.509(14) . ?
O5 O6 1.484(12) . ?
O8 O12 1.540(13) . ?
O10 O14 1.495(12) . ?
O16 O18 1.495(13) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 112.2(3) . . ?
O16 Ta1 O18 44.1(4) . . ?
O16 Ta1 O24 121.9(4) . . ?
O16 Ta1 O25 91.8(4) . . ?
O16 Ta1 O30 78.0(4) . . ?
O16 Ta1 O33 149.2(3) . . ?
O18 Ta1 Ta3 153.4(3) . . ?
O18 Ta1 O24 77.8(4) . . ?
O18 Ta1 O25 87.7(4) . . ?
O18 Ta1 O30 122.0(4) . . ?
O18 Ta1 O33 161.8(3) . . ?
O22 Ta1 Ta3 95.6(3) . . ?
O22 Ta1 O16 98.1(4) . . ?
O22 Ta1 O18 99.7(4) . . ?
O22 Ta1 O24 89.1(4) . . ?
O22 Ta1 O25 170.1(4) . . ?
O22 Ta1 O30 90.9(4) . . ?
O22 Ta1 O33 90.7(3) . . ?
O24 Ta1 Ta3 124.3(2) . . ?
O24 Ta1 O25 86.0(3) . . ?
O24 Ta1 O30 159.8(3) . . ?
O25 Ta1 Ta3 80.2(2) . . ?
O25 Ta1 O30 90.7(3) . . ?
O30 Ta1 Ta3 35.6(2) . . ?
O33 Ta1 Ta3 37.2(2) . . ?
O33 Ta1 O24 87.5(3) . . ?
O33 Ta1 O25 80.5(3) . . ?
O33 Ta1 O30 72.3(3) . . ?
O5 Ta2 Ta3 111.9(3) . . ?
O5 Ta2 O6 43.9(4) . . ?
O5 Ta2 O9 120.9(4) . . ?
O5 Ta2 O27 88.8(4) . . ?
O5 Ta2 O32 77.4(4) . . ?
O5 Ta2 O33 147.7(3) . . ?
O6 Ta2 Ta3 153.1(3) . . ?
O6 Ta2 O9 77.0(4) . . ?
O6 Ta2 O27 87.2(4) . . ?
O6 Ta2 O32 121.2(4) . . ?
O6 Ta2 O33 159.8(3) . . ?
O9 Ta2 Ta3 124.4(3) . . ?
O9 Ta2 O27 85.1(4) . . ?
O9 Ta2 O32 159.8(4) . . ?
O9 Ta2 O33 87.7(3) . . ?
O26 Ta2 Ta3 93.1(3) . . ?
O26 Ta2 O5 102.0(4) . . ?
O26 Ta2 O6 102.9(4) . . ?
O26 Ta2 O9 92.2(4) . . ?
O26 Ta2 O27 168.7(4) . . ?
O26 Ta2 O32 91.9(4) . . ?
O26 Ta2 O33 90.7(3) . . ?
O27 Ta2 Ta3 79.6(2) . . ?
O32 Ta2 Ta3 35.6(2) . . ?
O32 Ta2 O27 87.2(3) . . ?
O33 Ta2 Ta3 37.0(2) . . ?
O33 Ta2 O27 78.2(3) . . ?
O33 Ta2 O32 72.5(3) . . ?
Ta1 Ta3 Ta2 72.575(15) . . ?
Ta1 Ta3 K1 126.00(6) . . ?
Ta2 Ta3 K1 98.73(8) . . ?
O8 Ta3 Ta1 160.4(3) . . ?
O8 Ta3 Ta2 119.6(3) . . ?
O8 Ta3 K1 41.3(3) . . ?
O8 Ta3 O12 45.9(4) . . ?
O8 Ta3 O20 86.5(4) . . ?
O8 Ta3 O30 129.0(4) . . ?
O8 Ta3 O32 83.4(4) . . ?
O8 Ta3 O33 156.1(4) . . ?
O12 Ta3 Ta1 119.1(3) . . ?
O12 Ta3 Ta2 163.3(3) . . ?
O12 Ta3 K1 65.0(3) . . ?
O12 Ta3 O20 89.3(4) . . ?
O12 Ta3 O30 83.5(4) . . ?
O12 Ta3 O32 129.1(4) . . ?
O12 Ta3 O33 155.4(3) . . ?
O19 Ta3 Ta1 98.9(3) . . ?
O19 Ta3 Ta2 93.2(3) . . ?
O19 Ta3 K1 135.1(3) . . ?
O19 Ta3 O8 95.7(4) . . ?
O19 Ta3 O12 96.3(4) . . ?
O19 Ta3 O20 173.9(4) . . ?
O19 Ta3 O30 95.4(4) . . ?
O19 Ta3 O32 91.2(4) . . ?
O19 Ta3 O33 91.6(3) . . ?
O20 Ta3 Ta1 80.3(2) . . ?
O20 Ta3 Ta2 80.8(2) . . ?
O20 Ta3 K1 45.9(2) . . ?
O20 Ta3 O33 84.2(3) . . ?
O30 Ta3 Ta1 36.7(2) . . ?
O30 Ta3 Ta2 109.2(2) . . ?
O30 Ta3 K1 120.4(3) . . ?
O30 Ta3 O20 87.6(3) . . ?
O30 Ta3 O32 145.8(4) . . ?
O30 Ta3 O33 72.6(3) . . ?
O32 Ta3 Ta1 109.2(2) . . ?
O32 Ta3 Ta2 36.8(2) . . ?
O32 Ta3 K1 74.5(3) . . ?
O32 Ta3 O20 83.5(3) . . ?
O32 Ta3 O33 73.7(3) . . ?
O33 Ta3 Ta1 36.4(2) . . ?
O33 Ta3 Ta2 37.0(2) . . ?
O33 Ta3 K1 122.8(2) . . ?
Ta6 Ta4 Cs1 94.02(3) . . ?
O10 Ta4 Ta6 155.8(3) . . ?
O10 Ta4 Cs1 63.2(3) . . ?
O10 Ta4 O13 88.9(4) . . ?
O10 Ta4 O15 78.9(4) . . ?
O10 Ta4 O29 121.9(4) . . ?
O10 Ta4 O31 163.4(3) . . ?
O13 Ta4 Ta6 80.5(2) . . ?
O13 Ta4 Cs1 48.3(2) . . ?
O14 Ta4 Ta6 113.8(3) . . ?
O14 Ta4 Cs1 42.6(3) . . ?
O14 Ta4 O10 44.0(4) . . ?
O14 Ta4 O13 89.9(4) . . ?
O14 Ta4 O15 122.9(4) . . ?
O14 Ta4 O29 77.9(4) . . ?
O14 Ta4 O31 150.0(3) . . ?
O15 Ta4 Ta6 121.4(2) . . ?
O15 Ta4 Cs1 117.1(2) . . ?
O15 Ta4 O13 85.5(3) . . ?
O15 Ta4 O29 158.0(4) . . ?
O22 Ta4 Ta6 97.4(3) . . ?
O22 Ta4 Cs1 137.1(3) . . ?
O22 Ta4 O10 94.9(4) . . ?
O22 Ta4 O13 174.5(4) . . ?
O22 Ta4 O14 95.6(4) . . ?
O22 Ta4 O15 91.4(4) . . ?
O22 Ta4 O29 93.6(4) . . ?
O22 Ta4 O31 91.9(3) . . ?
O29 Ta4 Ta6 36.7(2) . . ?
O29 Ta4 Cs1 72.1(2) . . ?
O29 Ta4 O13 87.8(3) . . ?
O31 Ta4 Ta6 36.3(2) . . ?
O31 Ta4 Cs1 119.9(2) . . ?
O31 Ta4 O13 83.5(3) . . ?
O31 Ta4 O15 85.8(3) . . ?
O31 Ta4 O29 72.6(3) . . ?
O2 Ta5 Ta6 135.5(3) . . ?
O2 Ta5 O17 98.4(4) . . ?
O2 Ta5 O23 117.3(4) . . ?
O2 Ta5 O26 79.3(4) . . ?
O2 Ta5 O31 165.8(4) . . ?
O11 Ta5 Ta6 127.8(3) . . ?
O11 Ta5 O2 44.2(4) . . ?
O11 Ta5 O17 95.9(4) . . ?
O11 Ta5 O23 73.2(4) . . ?
O11 Ta5 O26 123.2(4) . . ?
O11 Ta5 O31 149.4(4) . . ?
O17 Ta5 Ta6 125.1(2) . . ?
O17 Ta5 O23 81.3(3) . . ?
O17 Ta5 O31 85.5(3) . . ?
O23 Ta5 Ta6 81.9(2) . . ?
O26 Ta5 Ta6 93.2(2) . . ?
O26 Ta5 O17 86.2(3) . . ?
O26 Ta5 O23 160.5(3) . . ?
O26 Ta5 O31 87.4(3) . . ?
O28 Ta5 Ta6 36.2(3) . . ?
O28 Ta5 O2 100.2(4) . . ?
O28 Ta5 O11 99.2(4) . . ?
O28 Ta5 O17 161.3(4) . . ?
O28 Ta5 O23 92.6(4) . . ?
O28 Ta5 O26 94.5(4) . . ?
O28 Ta5 O31 75.9(4) . . ?
O31 Ta5 Ta6 39.8(2) . . ?
O31 Ta5 O23 76.8(3) . . ?
Ta5 Ta6 Ta4 74.822(16) . . ?
O3 Ta6 Ta4 119.1(3) . . ?
O3 Ta6 Ta5 160.6(3) . . ?
O3 Ta6 O21 87.4(4) . . ?
O3 Ta6 O28 128.7(4) . . ?
O3 Ta6 O29 83.5(4) . . ?
O3 Ta6 O31 154.4(4) . . ?
O7 Ta6 Ta4 159.8(3) . . ?
O7 Ta6 Ta5 117.9(3) . . ?
O7 Ta6 O3 44.9(4) . . ?
O7 Ta6 O21 86.3(4) . . ?
O7 Ta6 O28 84.0(4) . . ?
O7 Ta6 O29 127.9(4) . . ?
O7 Ta6 O31 157.9(4) . . ?
O19 Ta6 Ta4 96.7(3) . . ?
O19 Ta6 Ta5 97.1(3) . . ?
O19 Ta6 O3 94.6(4) . . ?
O19 Ta6 O7 97.1(4) . . ?
O19 Ta6 O21 176.6(3) . . ?
O19 Ta6 O28 96.3(4) . . ?
O19 Ta6 O29 92.7(4) . . ?
O19 Ta6 O31 91.7(3) . . ?
O21 Ta6 Ta4 80.0(2) . . ?
O21 Ta6 Ta5 81.7(2) . . ?
O28 Ta6 Ta4 109.1(3) . . ?
O28 Ta6 Ta5 34.5(3) . . ?
O28 Ta6 O21 84.5(4) . . ?
O28 Ta6 O29 145.4(4) . . ?
O28 Ta6 O31 74.9(3) . . ?
O29 Ta6 Ta4 36.5(2) . . ?
O29 Ta6 Ta5 111.3(2) . . ?
O29 Ta6 O21 84.8(3) . . ?
O31 Ta6 Ta4 35.4(2) . . ?
O31 Ta6 Ta5 40.5(2) . . ?
O31 Ta6 O21 85.3(3) . . ?
O31 Ta6 O29 71.5(3) . . ?
O1 Gd1 Cs1 47.6(2) . 1_655 ?
O1 Gd1 O34 117.4(3) . . ?
O1 Gd1 O35 143.9(3) . . ?
O1 Gd1 O36 142.3(3) . . ?
O1 Gd1 O42 75.2(4) . . ?
O4 Gd1 Cs1 95.6(2) . 1_655 ?
O4 Gd1 O1 76.6(3) . . ?
O4 Gd1 O34 72.2(3) . . ?
O4 Gd1 O35 75.9(3) . . ?
O4 Gd1 O36 139.8(3) . . ?
O4 Gd1 O37 83.8(4) . . ?
O4 Gd1 O42 146.0(4) . . ?
O4 Gd1 O43 116.1(4) . . ?
O34 Gd1 Cs1 163.7(3) . 1_655 ?
O34 Gd1 O35 75.2(4) . . ?
O34 Gd1 O42 138.7(4) . . ?
O35 Gd1 Cs1 113.0(3) . 1_655 ?
O36 Gd1 Cs1 118.1(3) . 1_655 ?
O36 Gd1 O34 77.5(4) . . ?
O36 Gd1 O35 71.2(4) . . ?
O36 Gd1 O42 72.5(4) . . ?
O37 Gd1 Cs1 41.1(3) . 1_655 ?
O37 Gd1 O1 82.2(4) . . ?
O37 Gd1 O34 143.1(4) . . ?
O37 Gd1 O35 72.0(4) . . ?
O37 Gd1 O36 106.7(4) . . ?
O37 Gd1 O42 74.0(4) . . ?
O42 Gd1 Cs1 51.0(3) . 1_655 ?
O42 Gd1 O35 119.2(4) . . ?
O43 Gd1 Cs1 103.5(3) . 1_655 ?
O43 Gd1 O1 73.8(4) . . ?
O43 Gd1 O34 73.6(4) . . ?
O43 Gd1 O35 140.4(4) . . ?
O43 Gd1 O36 78.7(4) . . ?
O43 Gd1 O37 143.2(4) . . ?
O43 Gd1 O42 73.2(4) . . ?
O20 Se1 O25 100.4(4) . . ?
O27 Se1 O20 102.2(4) . . ?
O27 Se1 O25 104.5(4) . . ?
O13 Se2 Cs1 48.2(3) . . ?
O13 Se2 O21 101.2(4) . . ?
O13 Se2 O23 103.6(4) . . ?
O21 Se2 Cs1 88.8(3) . . ?
O23 Se2 Cs1 151.7(3) . . ?
O23 Se2 O21 101.8(4) . . ?
O4 Se3 O15 99.1(4) . . ?
O4 Se3 O17 99.3(4) . . ?
O15 Se3 O17 99.9(4) . . ?
O1 Se4 Cs1 57.0(3) . 1_655 ?
O1 Se4 O9 100.2(5) . . ?
O1 Se4 O24 101.0(4) . . ?
O9 Se4 Cs1 45.3(3) . 1_655 ?
O24 Se4 Cs1 116.2(3) . 1_655 ?
O24 Se4 O9 97.9(4) . . ?
O1 Cs1 O42 48.8(3) 1_455 1_455 ?
O6 Cs1 O1 90.2(2) 1_455 1_455 ?
O6 Cs1 O35 47.8(2) 1_455 4_475 ?
O6 Cs1 O42 139.0(3) 1_455 1_455 ?
O7 Cs1 O1 113.7(2) 4_576 1_455 ?
O7 Cs1 O6 107.9(2) 4_576 1_455 ?
O7 Cs1 O9 124.9(3) 4_576 1_455 ?
O7 Cs1 O13 60.6(2) 4_576 . ?
O7 Cs1 O14 110.0(3) 4_576 . ?
O7 Cs1 O35 60.1(3) 4_576 4_475 ?
O7 Cs1 O37 58.8(3) 4_576 1_455 ?
O7 Cs1 O40 131.2(3) 4_576 . ?
O7 Cs1 O41 71.1(3) 4_576 . ?
O7 Cs1 O42 90.9(3) 4_576 1_455 ?
O9 Cs1 O1 45.2(2) 1_455 1_455 ?
O9 Cs1 O6 45.4(2) 1_455 1_455 ?
O9 Cs1 O13 153.3(2) 1_455 . ?
O9 Cs1 O14 123.7(2) 1_455 . ?
O9 Cs1 O35 79.3(3) 1_455 4_475 ?
O9 Cs1 O37 84.3(3) 1_455 1_455 ?
O9 Cs1 O40 77.4(3) 1_455 . ?
O9 Cs1 O41 140.8(3) 1_455 . ?
O9 Cs1 O42 94.0(3) 1_455 1_455 ?
O13 Cs1 O1 161.4(2) . 1_455 ?
O13 Cs1 O6 108.3(2) . 1_455 ?
O13 Cs1 O35 83.7(2) . 4_475 ?
O13 Cs1 O42 112.6(3) . 1_455 ?
O14 Cs1 O1 122.9(2) . 1_455 ?
O14 Cs1 O6 109.3(2) . 1_455 ?
O14 Cs1 O13 52.3(2) . . ?
O14 Cs1 O35 123.6(2) . 4_475 ?
O14 Cs1 O37 140.5(3) . 1_455 ?
O14 Cs1 O40 55.9(3) . . ?
O14 Cs1 O41 65.6(3) . . ?
O14 Cs1 O42 97.1(3) . 1_455 ?
O35 Cs1 O1 109.4(2) 4_475 1_455 ?
O35 Cs1 O42 135.2(3) 4_475 1_455 ?
O37 Cs1 O1 55.2(3) 1_455 1_455 ?
O37 Cs1 O6 110.2(3) 1_455 1_455 ?
O37 Cs1 O13 115.0(3) 1_455 . ?
O37 Cs1 O35 85.7(3) 1_455 4_475 ?
O37 Cs1 O42 49.5(3) 1_455 1_455 ?
O40 Cs1 O1 111.3(3) . 1_455 ?
O40 Cs1 O6 54.0(3) . 1_455 ?
O40 Cs1 O13 81.5(3) . . ?
O40 Cs1 O35 88.1(3) . 4_475 ?
O40 Cs1 O37 161.5(3) . 1_455 ?
O40 Cs1 O42 134.0(3) . 1_455 ?
O41 Cs1 O1 96.2(3) . 1_455 ?
O41 Cs1 O6 173.3(3) . 1_455 ?
O41 Cs1 O13 65.2(3) . . ?
O41 Cs1 O35 130.6(3) . 4_475 ?
O41 Cs1 O37 75.2(3) . 1_455 ?
O41 Cs1 O40 121.4(4) . . ?
O41 Cs1 O42 47.5(3) . 1_455 ?
O49 Cs1 O1 58.4(6) 3_566 1_455 ?
O49 Cs1 O6 81.7(6) 3_566 1_455 ?
O49 Cs1 O7 168.3(6) 3_566 4_576 ?
O49 Cs1 O9 57.2(6) 3_566 1_455 ?
O49 Cs1 O13 123.7(6) 3_566 . ?
O49 Cs1 O14 71.8(6) 3_566 . ?
O49 Cs1 O35 129.2(6) 3_566 4_475 ?
O49 Cs1 O37 112.1(6) 3_566 1_455 ?
O49 Cs1 O40 59.8(6) 3_566 . ?
O49 Cs1 O41 100.2(6) 3_566 . ?
O49 Cs1 O42 77.4(6) 3_566 1_455 ?
O8 K1 Ta3 27.16(19) . . ?
O8 K1 O11 76.7(3) . 4_575 ?
O8 K1 O20 57.1(3) . . ?
O8 K1 O41 70.9(3) . 1_554 ?
O8 K1 O44 127.9(4) . 3_666 ?
O8 K1 O45 149.9(4) . . ?
O8 K1 O50 86.5(5) . . ?
O11 K1 Ta3 81.0(2) 4_575 . ?
O11 K1 O50 157.7(5) 4_575 . ?
O20 K1 Ta3 30.42(17) . . ?
O20 K1 O11 94.5(3) . 4_575 ?
O20 K1 O41 127.8(3) . 1_554 ?
O20 K1 O50 63.9(5) . . ?
O41 K1 Ta3 97.4(3) 1_554 . ?
O41 K1 O11 67.3(3) 1_554 4_575 ?
O41 K1 O50 120.9(5) 1_554 . ?
O44 K1 Ta3 101.1(3) 3_666 . ?
O44 K1 O11 111.6(4) 3_666 4_575 ?
O44 K1 O20 70.8(3) 3_666 . ?
O44 K1 O41 161.1(4) 3_666 1_554 ?
O44 K1 O50 67.8(5) 3_666 . ?
O45 K1 Ta3 151.1(3) . . ?
O45 K1 O11 75.2(4) . 4_575 ?
O45 K1 O20 135.7(4) . . ?
O45 K1 O41 88.3(4) . 1_554 ?
O45 K1 O44 73.5(4) . 3_666 ?
O45 K1 O50 123.4(5) . . ?
O46 K1 Ta3 131.9(3) . . ?
O46 K1 O8 117.3(4) . . ?
O46 K1 O11 134.9(4) . 4_575 ?
O46 K1 O20 129.8(4) . . ?
O46 K1 O41 77.2(4) . 1_554 ?
O46 K1 O44 93.2(4) . 3_666 ?
O46 K1 O45 76.9(4) . . ?
O46 K1 O50 66.0(5) . . ?
O50 K1 Ta3 77.5(4) . . ?
Gd1 O1 Cs1 102.1(3) . 1_655 ?
Se4 O1 Gd1 128.3(5) . . ?
Se4 O1 Cs1 99.8(4) . 1_655 ?
O11 O2 Ta5 67.8(6) . . ?
O7 O3 Ta6 67.2(5) . . ?
Se3 O4 Gd1 176.7(6) . . ?
O6 O5 Ta2 68.8(5) . . ?
Ta2 O6 Cs1 116.0(3) . 1_655 ?
O5 O6 Ta2 67.2(5) . . ?
O5 O6 Cs1 175.3(6) . 1_655 ?
Ta6 O7 Cs1 147.7(5) . 4_575 ?
O3 O7 Ta6 67.9(5) . . ?
O3 O7 Cs1 130.7(6) . 4_575 ?
Ta3 O8 K1 111.5(4) . . ?
O12 O8 Ta3 67.7(5) . . ?
O12 O8 K1 108.7(6) . . ?
Ta2 O9 Cs1 121.6(4) . 1_655 ?
Se4 O9 Ta2 123.2(5) . . ?
Se4 O9 Cs1 112.0(4) . 1_655 ?
O14 O10 Ta4 67.6(5) . . ?
Ta5 O11 K1 148.1(5) . 4_576 ?
O2 O11 Ta5 68.0(6) . . ?
O2 O11 K1 124.6(7) . 4_576 ?
O8 O12 Ta3 66.5(5) . . ?
Ta4 O13 Cs1 103.9(3) . . ?
Se2 O13 Ta4 129.5(5) . . ?
Se2 O13 Cs1 109.6(4) . . ?
Ta4 O14 Cs1 112.4(4) . . ?
O10 O14 Ta4 68.4(5) . . ?
O10 O14 Cs1 106.5(6) . . ?
Se3 O15 Ta4 136.5(5) . . ?
O18 O16 Ta1 68.7(5) . . ?
Se3 O17 Ta5 131.0(5) . . ?
O16 O18 Ta1 67.1(5) . . ?
Ta3 O19 Ta6 164.1(5) . . ?
Ta3 O20 K1 103.7(3) . . ?
Se1 O20 Ta3 126.6(4) . . ?
Se1 O20 K1 121.9(4) . . ?
Se2 O21 Ta6 125.6(5) . . ?
Ta1 O22 Ta4 164.5(5) . . ?
Se2 O23 Ta5 131.0(5) . . ?
Se4 O24 Ta1 122.8(5) . . ?
Se1 O25 Ta1 131.3(5) . . ?
Ta2 O26 Ta5 167.7(5) . . ?
Se1 O27 Ta2 131.2(5) . . ?
Ta5 O28 Ta6 109.3(4) . . ?
Ta4 O29 Ta6 106.8(4) . . ?
Ta3 O30 Ta1 107.7(4) . . ?
Ta4 O31 Ta5 146.8(4) . . ?
Ta4 O31 Ta6 108.3(4) . . ?
Ta6 O31 Ta5 99.7(3) . . ?
Ta3 O32 Ta2 107.7(4) . . ?
Ta1 O33 Ta2 143.9(4) . . ?
Ta1 O33 Ta3 106.4(4) . . ?
Ta3 O33 Ta2 106.0(3) . . ?
Gd1 O35 Cs1 160.6(4) . 4_676 ?
Gd1 O37 Cs1 110.1(4) . 1_655 ?
K1 O41 Cs1 148.7(5) 1_556 . ?
Gd1 O42 Cs1 97.4(4) . 1_655 ?

_olex2_submission_special_instructions 'No special instructions were received'
